Multi-scale constitutive model and computational

framework for the design of ultra-high strength,

high toughness steels

Su Hao

a,b,

*

,Wing Kam Liu

b,

*

,Brian Moran

b

,Franck Vernerey

b

,

Gregory B.Olson

a

a

Department of Materials and Science Engineering,Northwestern University,2145 Sheridan Road,

Evanston,IL 60208-3111,USA

b

Department of Mechanical Engineering,The Technological Institute,Northwestern University,2145 Sheridan Road,Evanston,

IL 60208-3111,USA

Received 5 June 2003;received in revised form 16 October 2003;accepted 2 December 2003

Abstract

A multi-scale hierarchical constitutive model is developed for establishing the relationship between quantum

mechanical,micromechanical,and overall strength/toughness properties in steel design.Focused on the design of ultra-

high strength,high toughness steels,a two-level cell model is used to represent two groups of hard particles (inclusions)

in an alloy matrix which is characteristic of such Fe-based alloys.Primary inclusion particles,which are greater than a

micron in size,are handled by a microcell.Secondary inclusion particles which are tens of nanometers in size are

modeled by a sub-microcell.In the sub-microcell,the matrix constitutive behavior is given by quantum mechanics

computation of bcc-iron calibrated according to experiments.In the microcell,the matrix constitutive behavior is given

by the stress–strain response of the sub-microcell,characterized by a plastic ﬂow potential based on the numerical

simulation of the representative cell.In turn,the plastic ﬂow potential generated by the stress–strain response of the

microcell is used as the constitutive response at the continuummacro level for simulation of ductile fracture and for the

assessments of toughness.The interfacial debonding between the matrix and the primary and the secondary inclusion

particles are modeled using decohesion potentials computed through quantum mechanics calculation together with a

mechanical model of normal separation and gliding induced dislocation,which also provides quantitative explanations

why practice strength of a steel is much lower than the atomic separation force and how plasticity occurs in steels.

The ductile fracture simulations on an ASTMstandard center cracked specimen lead to the generation,for the ﬁrst

time,of a toughness,strength,adhesion diagram based on computer simulation and which establishes the relationship

between alloy matrix strength,interfacial decohesion energy,and fracture toughness.

2004 Elsevier B.V.All rights reserved.

Keywords:Multi-scale multi-physics;Multiple scales;Plasticity;Constitutive law;Fracture toughness;Steel design;Materials design;

Particle dynamics;MD

*

Corresponding authors.Address:Department of Mechanical Engineering,The Technological Institute,Northwestern University,

2145 Sheridan Road,Evanston,IL 60208-3111,USA.Tel.:+847-491-7094;fax:+847-491-3915.

E-mail addresses:suhao@northwestern.edu,suhao1@yahoo.com(S.Hao),w-liu@northwestern.edu (W.K.Liu),b-moran@north-

western.edu (B.Moran),f-vernerey@northwestern.edu (F.Vernerey),olson@igor.tech.northwestern.edu (G.B.Olson).

0045-7825/$ - see front matter 2004 Elsevier B.V.All rights reserved.

doi:10.1016/j.cma.2003.12.026

Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908

www.elsevier.com/locate/cma

1.Introduction

One of the principal objectives of micro/nanomechanics of materials is to account for the observed

phenomena and properties of macroscopic solid bodies,such as strength and fracture toughness of steels,

on the basis of the quantum mechanical theory of the behavior of atomic particles.Success will have been

achieved when it becomes possible to calculate the quantities that describe the constitution of materials and

their response to alterations of macroscopic mechanical boundary conditions from the knowledge of the

component elements and their hierarchical structures from atomistic–electronic scales to micro- and

macroscales.This is particularly important for steel design.

For this purpose,the diﬃculties and complexity originate in the substantial diﬀerences in philosophy and

viewpoints between conventional continuummechanics and quantumtheory.In the former,the solution of

a boundary value problem is uniquely determined based on Newtons laws when initial and boundary

conditions are given;whereas the Heisenberg uncertainty principle,the cornerstone of quantummechanics,

indicates that motion of a particle is characterized by wave solutions of Sch

€

odingers equation and the

intensity of wave solutions deﬁnes the ‘‘probability density’’ for the position of this particle.For mechanical

engineers,the challenges lie in how to establish the relationship between a continuum mechanical system

and its atomistic–electronic structure and how to constitute a uniﬁed framework that bridges the mecha-

nisms from diﬀerent scales.These are the key-issues in the ONR project ‘‘cybersteel2020’’ [1] towards the

predictive design of novel steels to combine high strength and fracture toughness.

Both strength and fracture toughness are the key property-indices for steels.Although advanced tech-

nology currently provides many ways to achieve either high strength or high toughness,respectively,in steel

through manufacturing processes,it remains a challenge to achieve both of them simultaneously.This is

because the toughness characterizes the capability of a material against fracture at a crack tip local.The

diﬀerence between the local and the global properties reﬂects the natural heterogeneity of the micro-

structure of steels.The design of steels seeks to achieve desirable micro/nanostructures with optimized

properties through alloy component/phase selection and metallurgical processes based on quantitative

understanding of controlling mechanisms and the relationships among these at diﬀerent scales.

In this paper,a bottom-up computational methodology has been proposed to establish a hierarchical

multi-physics constitutive model that builds up the relationships among the macroscale properties,micro-

and sub-microstructures,and atomistic failure modes for steels.To this end,new models and computa-

tional schemes have been developed.The innovations presented here can be summarized as follows:

1.We propose an atomistic adhesion model that counts for both the separation normal to newly created

interfaces and gliding induced dislocations.The normal separation is described as a creation of empty

sites,which may trigger gliding induced dislocation that translates the short-ranged covalent binding

force into a long-ranged decohesion law.Rices criterion [2] is used to determine these two competing

mechanisms.The computed results provide a quantitative explanation why the practical strength of a

steel is much lower than the prediction of atomic separation and how plasticity occurs in steel.

2.A ﬁrst-principle based ab initio computation has been performed to calculate the generalized fault en-

ergy against dislocation induced sliding in a bcc-Fe crystal.

3.A‘‘Quasi-particle dynamics approach’’ has been developed,which transforms an atomistic systeminto a

‘‘particle system’’ while maintaining intrinsic structural properties such as crystal elastic constants and

molecular dynamic kinetics.Each particle can be a ‘‘super-atom’’ containing several atoms,or represents

an inclusion particle,depending upon the scales of interest.As the particle systemcan have fewer degrees

of freedom than the atomistic system,the method can be used for bridging atomistic and continuum

scales.

4.A hierarchical multi-physics computational constitutive model has been developed based on a uniﬁed

thermodynamic framework.This model is applied in a computation procedure,which is named as a

1866 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908

‘‘ductile fracture simulator’’ by the authors,to support quantitative tradeoﬀ analysis in microstructural

optimization for fracture toughness.

5.A toughness–strength–adhesion diagram has been obtained for steel design,which establishes the rela-

tionship among alloy matrix strength,inclusion adhesion interfacial energy and fracture toughness.To

the authors knowledge this is the ﬁrst computer generated design diagram for engineering application.

This paper is organized as follows:In Section 2 we introduce the hierarchical model.Section 3 describes

the quantum physics analysis and the bridge to continuum mechanics.The Quasi-particle dynamics ap-

proach is introduced in Section 4.A uniﬁed multi-physics thermodynamic framework in continuum

mechanics and a two-level cell representation at sub-micro- and microscales are derived in Section 5,which

lead to a hierarchical constitutive model.Simulations of crack propagation and fracture toughness are

presented in Section 6.As a conclusion,a toughness–strength–adhesion diagram is developed.This dia-

gram,together with the hierarchical constitutive model and computational procedure,constitute the

‘‘ductile fracture simulator’’ presented in Section 7.

2.Methodology and approach

Like all conventional materials,steels are heterogeneous in-nature.A modern ultra-high strength steel

generally consists of an alloy matrix with several levels of dispersed small hard inclusion particles (see Fig.

1).Interfacial strength between the diﬀerent phases plays an important role in the strength and toughness of

steels.

For the ultra-high strength steels considered here,dispersions of hard particles occur at two distinct

scales:primary particles (such as TiN,MgS,Fe

3

C) are typically on the order of microns in size;and sec-

ondary particles (such as TiC,TiC

2

S and M

2

C compounds) are on the order of tens of nanometers in size.

To develop a macroscopic constitutive model for ultra-high strength,high toughness steel,we propose a

multi-physics approach based on hierarchical unit cell representations of the primary particles and sec-

ondary particles.A quantum mechanical analysis is performed to determine the constitutive relations for

Fig.1.A TEM micrograph of the fracture surface of a ultra-high-strength steel (with the courtesy of Prof.G.Kruass,School of

Corolado of Mine).

S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1867

the iron matrix and the interfacial behavior between the matrix and the inclusions,leading in turn to the

continuum mechanics decohesion potentials for diﬀerent interfaces and alloy matrices.A continuum

mechanics analysis is applied in the unit cell representation with primary particles,which we call

‘‘microscale cell model’’.A ‘‘Quasi-particle dynamics approach’’ is developed for the cell representation

with secondary particles,which is termed ‘‘sub-microcell model’’.At the quantum scale,the sub-atomic

primitive cells are applied in interfacial separation and bulk iron matrix adhesion analyses.Thus,the

proposed approach links mechanisms from quantum-atomistic scales and micro/sub-microscales to the

scale of a laboratory fracture toughness specimen,as demonstrated in the ﬂow chart of Fig.2a and brieﬂy

illustrated in Fig.2b.

In Fig.2b and in the following analysis,r

ij

and e

ij

denote the stresses and strains at the sub-microscale.

The sub-microscale cell model homogenizes r

ij

and e

ij

into the microscale stress and strain which are de-

noted by R

micro

ij

and E

micro

ij

,respectively;and a microscale plastic potential U

micro

is developed.By repeating

this procedure the macroscale stress–strain:R

ij

,E

ij

,and the corresponding macroscale plastic potential

U

macro

,are obtained,which is applied to the laboratory specimen to fracture simulation.

In the following section,we begin with a description of the crystal separation behavior and the

underlying quantum mechanical consideration,leading to a continuum mechanics force–separation law.

3.Interfacial separation:from quantum mechanics to continuum mechanics

3.1.Interfacial separation:from quantum nanomechanics to continuum micromechanics

For a metallic or intermetallic systemwhere each atomhas a suﬃcient number of electrons,the Thomas-

Fermi [3,4] model is applicable.This model approximates the system as a combination of static atomic

cores that formthe crystal and an electronic gas that ﬁlls the space among the atoms.Hohenberg and Kohn

[5] and Kohn and Shams [6] theorems indicate that the ground-state energy of such a many body system,

which is an eigenvalue of the corresponding wave solution of the Schr

€

odinger equation,is determined by

electron density distribution.Based on the augmented plane wave method introduced by Slater [7],various

numerical methods have been developed to determine the electron density distribution,e.g.[8–11].Among

them,the full-potential spin-polarized linear augmented plane wave (FLAPW) [12] is presently considered

to be the most accurate scheme as it holds the fewest approximations.

Macroscopic fracture of a crystal is a process whereby atomic aggregates are split into two parts.For a

defect-free system where separation is normal to the newly created surfaces,Rose et al.[13] found that the

binding energy obeys an approximate ‘‘universal relation’’ of the form

E

N

ðk

N

Þ ¼ ½Eðk

N0

Þ Eð1Þ E

N

k

N

l

TF

;

k

N0

l

TF

;ð3:1Þ

where E

N

ðk

N

Þ is the binding energy;k

N

is the normal separation and k

N0

is the normal separation at the

equilibrium state;Eðk

N0

Þ and Eð1Þ are the total ground-state energies of the system at k

N0

and k

N

!1,

respectively;l

TF

is a scaling length which characterizes an atomic size and E

N

is function which describes the

shape of E

N

ðk

N

Þ.When the system is fully separated and no extra strain is imposed before and after this

separation,the change of the total ground-state energy is identical to the newly created surface energy,i.e.

2Ac

F

¼ Eðk

N0

Þ Eð1Þ;ð3:2Þ

where c

F

is the surface energy per unit area and A is the area of the newly created surfaces.

Real crystals may contain a variety of imperfections,e.g.impurity or interstitial atoms,vacant lattice

site,and dislocations.The normal separation (3.1) can be viewed as the creation of new vacant lattice sites,

1868 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908

Fig.2.(a) The ﬂow chart of the proposed approach.(b) An illustration of the proposed hierarchical model that links a:the quantum

scale,b:sub-microscale,c:microscale,d:macroscale.

S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1869

which may trigger other defects,such as the motion of dislocations along interacting slip planes.Rices

criterion [2] states that dislocation motion will be activated when the energy barrier,c

US

,against unstable

sliding is smaller than the cleavage surface energy,c

F

,which provides a basis for describing the competition

between these two mechanisms.The mathematical expression of Rices criterion is:

c

F

c

US

j

R

> 1;ð3:3Þ

where j

R

is a function of the average lattice elastic stress and the angle/between the slip-plane and the

newly-created surface,and j

R

< 1.When dislocation induced sliding occurs,the relation between the total

system energy E

S

and sliding separation k

S

per dislocation can be written as:

E

S

ðk

S

Þ ¼ c

US

E

S

ðk

S

;/Þ;ð3:4Þ

where E

S

ðk

S

;/Þ is a normalized function which describes the shape of E

S

ðk

S

Þ.

Weertman [14] studied a rectangular wave shape for E

S

ðk

S

;/Þ.Based on the Peierls concept for a

monoclinic crystals,an approximate expression for E

S

is suggested in [2]

E

S

¼ sin

4

pk

S

b

:ð3:5Þ

The relations (3.1)–(3.4) are fundamental equations of atomistic fracture.To obtain accurate values of c

F

and c

US

,and expressions for E

S

and E

N

,ﬁrst principle-based calculations are required which will be

introduced in the next section.The quantum mechanics formulation and the method used to obtain these

quantities are brieﬂy described in Appendix A.

In this paper the ﬁrst-principle calculations are used to compute the binding energy relations for the

following systems:

(1) iron matrix:normal adhesion and sliding;

(2) interfacial decohesion between alloy matrix and TiC

x

N

1x

particles (x ¼ 0:primary particle;x ¼ 1:sec-

ondary particle).

3.2.First-principle computations

The fundamentals of ﬁrst-principle computation are introduced in [8,11,12] based on density functional

theory [5,6].

The most important step of a ﬁrst-principle computation of a crystal is to set up the corresponding

geometrical model,i.e.the primitive cell of atomistic analysis.A density functional theory (DFT) based

computation requires the calculation of charge density distribution among atoms.It is crucial to design a

primitive cell that is able to represent the fundamental physics yet which contains suﬃciently small numbers

of atoms so as to be computationally treatable.

The starting point for designing an atomistic primitive cell in this study is presuming that the interested

atomic structures of iron and the Fe/TiC interface are much smaller than those geometrical parameters such

as particle/grain sizes,so that an iron crystal can be considered to be an inﬁnite slab of atoms and the Fe/

TiC interface can be considered to be the boundary between a semi-inﬁnite iron slab and semi-inﬁnite TiC

slab.Since interatomic forces (covalent binding forces) are short-range in nature,it is reasonable to design a

repeatable sub-atomic cell with the minimumrequisite number of atoms by using the periodic structure of a

crystal.

In the following analysis,we use ‘‘AkB’’ to denote the interface between crystal A and B.For example,

‘‘f001g

Fe

bcc

kf001g

TiC

fcc

’’ denotes the interface between a {0 01} surface of a bcc-Fe crystal and a {00 1}

surface of a (NaCl structured) fcc-TiC crystal,as shown in Fig.3a.

1870 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908

For a system such as the Fe/TiC interface shown in Fig.3a,the following failure modes may occur:

1.normal and sliding separations in Fe;

2.normal and sliding separations in the TiC;

3.Fe/TiC interfacial debonding.

The TiC,as a ceramic,has a much higher coherent strength than Fe [15],so the failure mode 2 is ex-

cluded in this analysis.

Both the normal separation and shear sliding in iron matrix have been studied in this paper.We have

computed the ½

1

11 shear fault energy on the ð1

11Þ plane,the normal separation of Fe–Ti site of the

f001g

Fe

bcc

kf001g

TiC

fcc

interface,and the separation normal to {11 1} plane in a perfect bcc-Fe crystal with

two-empty sites using the linearized augmented plane wave code based on [9].These computations,in

conjunction with the results from collaborators [16,17] and the literature [15,18],provide a clear picture of

decohesion process of the steel at the quantum scale.The details are given as follows.

3.2.1.Normal separation

3.2.1.1.Fe–Ti site at TiC–bcc-Fe interface.For the interface decohesion problem,the diﬃculty lies in the

anisotropic-nature of crystalline structures and the misﬁt in lattice constants between the two diﬀerent

crystals.It is well known that at roomtemperature Fe exists as a bcc crystal with a lattice constant of 0.287

nm [19] and TiC exists as a NaCl(fcc) structure with a lattice constant 0.4332 nm [15,20] (Fig.3a).The

challenge is to ﬁnd the sites which have the minimum lattice misﬁt and the strongest binding energy,thus

which form the most coherent junctions among the combinations of Fe–TiC interfacial structures.

For bcc-Fe,the distances from an atom to its most closest neighbors are 0.249 nm (between bcc corner

and center atoms),0.287 nm (the edge length of a cubic unit of bcc crystal),and 0.407 nm (between the

diagonal atoms pair on the surface of a cubic bcc unit).Obviously,the last one is the site with the minimum

misﬁt to the lattice constant (0.4332 nm) of the TiC.Hence,the f001g

Fe

bcc

kf001g

TiC

fcc

junction matches the

Fig.3.(a) Coherent TiC–Fe [1 00] interface;(b) top-down view ([0 0

1]) of the TiC/Fe interface with the neighbored Fe layer and TiC

layer where Fe atoms sit on the saddle point of TiC crystal.Fe–C site:the Fe crystal moves as indicated by the vector

a;Fe–Ti site:the

Fe crystal moves by the vector

b.

S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1871

most preferred binding surfaces of both sides with three possible arrangements:Fe–C site,Fe–Ti site,and

Fe–TiC saddle point site (see Fig.3b).

The study of the coherent Fe–TiC interface was ﬁrst performed by Freemans group [17] using FLAPW

[21].In this paper the simulation and calibration of (3.1) and (3.2) of the sub-atomic cell of

f001g

Fe

bcc

kf001g

TiC

fcc

decohesion is computed.The interfacial debonding energies are listed in Table 1.

It should be pointed out that the primitive model of Fig.3a actually represents the interface of a

periodically repeated Fe/TiC layered structure.The height of each layer is twice times of the atoms layers

plotted in the ﬁgure.In this primitive cell analysis the eﬀects of layer overlay are omitted.

3.2.1.2.Decohesion normal to (11 1) in bcc-iron.A sub-atomic cell is developed as illustrated in Fig.4a,

where the primitive vectors take the form

a ¼

^

x þ

^

y;

b ¼

^

y þ

^

z;

c ¼

^

x þ

^

y þ

^

z;ð3:6Þ

which are originated at ð

^

x;0;0Þ.Presuming the six outer surfaces of the cell to be rigid,periodic boundary

conditions are imposed on the two surfaces pairs:f0;y

b;z

cg and f

a;y

b;z

cg as well as fx

a;0;z

cg and

fx

a;

b;z

cg;where (x;y;z) are the coordinates deﬁned in the system f

a;

b;

cg.The surfaces fx

a;y

b;0g and

fx

a;y

b;

cg are enforced to move oppositely normal to the (1 11) plane.For the case with two-empty sites,

the two middle atoms marked with dark color inside are taken away.The sub-atomic cell is periodically

Table 1

Surface energies and equilibrium separations––results of ﬁrst principle calculations

Decohesion surface Interface 2c

F

(J/M

2

) k

N0

(nm) Source

f001g

Fe

bcc

kf001g

TiC

fcc

Fe–C site 3.82 0.213 [17]

f001g

Fe

bcc

kf001g

TiC

fcc

Fe–Ti site 0.61 0.361 This work (Fig.4b)

{11 1} Perfect 5.43 0.094 This work (Fig.4b)

{11 1} Perfect 5.38 0.0809 [18]

{11 1} Two-empty sites 1.1 0.241 This work (Fig.4b)

½

1

11 stacking fault Fe–Fe c

US

¼ 0:43 (J/M

2

) This work (Fig.6)

Fig.4.(a) Sub-atomic cell for {111} plane separation in bcc-iron crystal and (b) the computed energy-separation relations for three

cases.

1872 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908

reproducible throughout space.The 12 ·12·1 k-point mesh with Monkhorst and Pack scheme is applied in

the simulations.

3.2.1.3.Results of normal separation.The results are summarized in Table 1.The corresponding computed

energy-separation curves are plotted in Fig.4b.

3.2.2.Gliding induced dislocation

The stacking fault energy barrier c

US

is a crucial parameter for materials,as Eq.(3.3) indicates that the

ratio of

c

F

c

US

determines the mode of separation,which determines toughness.This is because at macroscale,

normal separation represents brittle fracture whereas atomistic sliding corresponding to plastic ﬂow.When

c

US

< c

F

,gliding induces dislocation motions.A dislocation core is an empty site that reduces the deco-

hesion energy signiﬁcantly when normal decohesion occurs,see Fig.4b and Table 1.

There is a considerable amount of research on ﬁrst principle-based simulations of stacking fault

mechanisms in fcc crystal,e.g.[22],whereas few results are reported for Fe-bcc crystals.In a bcc crystal,

sliding along {110} planes in the h111i direction is an often observed active screw dislocation pattern.

Because sliding may turn from one h111i direction to another,it usually moves along a zigzag path.A

½

1

11 fault is a possible composition of several zigzag motions.

In this paper,we study the ½

1

11 fault.The importance of this motion is that two such stacking faults

form a complete glide dislocation,i.e.:

a

2

½

1

11 þ

a

2

½111!a½001;ð3:7aÞ

where ‘‘a’’ is lattice constant.A ½

1

11 fault can be decomposed into the following three steps:

a

2

½

1

11!

a

8

½

1

10 þ

a

4

½

1

12 þ

a

8

½

1

10;ð3:7bÞ

which is formed by a zigzag path on the ð1

10Þ plane.It moves ﬁrst along the intersection of ð1

11Þ and

ð1

10Þ planes which is the line segment ½

1

10;then moves along the intersection of (1 11) and ð1

10Þ planes

which is the line segment ½

1

12 and ﬁnally back to the direction of line segment ½

1

10.In Fig.5,a primitive

cell representing the periodic repeating motion of (3.7b) is given.Its primitive vectors,which originate at

ð0;

^

y;

^

zÞ,take the form

a ¼

a

2

½

^

x

^

y þ

^

z;

b ¼

a

2

½

^

x þ

^

y þ

^

z;

c ¼

a

2

½ð1 qÞ

^

x ð1 qÞ

^

y gðqÞ

^

z;ð3:8Þ

Fig.5.The primitive cell for a [

1

11] dislocation.

S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1873

where q varies from 0 to 1,representing the gliding induced sliding;and

gðqÞ ¼

1 q < 0:25;

3 4q

2

0:256q < 0:75;

0 q P0:75:

8

>

>

<

>

>

:

The computed energy-sliding relation is plotted in Fig.6,which demonstrates the energy barrier c

US

for the

motion of

a

8

½

1

10 is about 0.31 J/M

2

and the c

US

for

a

4

½

1

12 is about 0.43 J/M

2

.

Recall Rices criterion (3.3)

c

F

c

US

j

R

ð/Þ > 1;

where j

R

ð/Þ 0:3.Comparing Fig.6 and the results listed in Table 1,we conclude that at the Fe–C site of

the TiC/Fe interface and in a perfect bcc-Fe matrix,relation (3.3) is satisﬁed so that sliding induced

separations dominate the decohesion process.Under these situations,fracture is ‘‘intrinsically’’ ductile.

Also from Table 1 we ﬁnd that point defects,such as vacancies,have a strong eﬀect on the fracture

mechanisms since they reduce the decohesion energy signiﬁcantly,and thus transform a ductile fracture to

brittle.

3.2.3.The ‘‘c plane’’ sliding

According to the diﬀerence in decohesion energy between the Fe–C site and the Fe–Ti site (see Table 1),

we obtain an estimate of (3.4) for the sliding tangential to the Fe–TiC interface,termed ‘‘c plane’’ sliding:

E

c

ðk

c

Þ ¼ A

S

sin

4

pk

cx

b

sin

4

pk

cy

b

;ð3:9Þ

where

A

S

¼

k

Nc

0

k

N

6

ðc

S

j

Fe–C

c

S

j

Fe–Ti

Þ;

k

Nc0

¼ 0:213 nm,b is taken as the average of the lattice constants of TiC (0.4332 nm) and Fe (0.407 nm);k

cx

,

k

cy

are the projections of k

c

onto the x- and y-axis in Fig.3b,respectively;when k

Sx

¼ k

Sy

¼ 0,it refers to the

Fe–C site.

Fig.6.The energy-dislocation core position curve of [

1

11] dislocation.

1874 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908

3.3.A proposed potential approach based on Needleman’s potential and quantum mechanics simulation

Needleman [23] developed an interface cohesive model that deﬁnes the normal traction ðr

N

Þ and tan-

gential traction ðr

T

Þ along the interface through a potential W

interface

r

N

¼

oW

interface

o½u

N

;r

T

¼

oW

interface

o½u

T

;ð3:10Þ

where ½u

N

,½u

T

are normal and tangential interfacial separations,respectively.An expression for U

i

is given

in [23] which is calibrated using experimental results [24].

In this study,we split the Needlemans potential into normal separation part W

N

and tangential part W

T

,

respectively

r

N

¼

oW

N

o½u

N

;r

T

¼

oW

T

o½u

T

:ð3:10aÞ

According to (3.1)–(3.4),we propose that the W

N

and W

T

take the forms of

W

N

¼ E

N

þj

slide

X

E

S

;W

T

¼ E

c

;ð3:11Þ

where E

N

is given in Table 1;E

c

is given by (3.9).

P

E

S

is the summation of sliding energy for all slip

systems except the c plane and j

slide

is a coeﬃcient to be determined;which will be discussed in the next

section.

3.4.Rescaling factor

The expression (3.11) is inconvenient for continuum mechanical analysis when no sliding occurs.This is

because (3.1) describes a process of covalent bond breaking which is very short-ranged.The corresponding

force usually becomes negligible when separation is greater than 1 nm,which is not an appropriated scale

for continuummechanics.On the other hand,it is also not trivial to compute the term‘‘j

slide

P

E

S

’’ in (3.11)

accurately.

The previous analysis indicates that iron is ‘‘intrinsically ductile’’.When normal separation consorts with

a dislocation induced sliding,the short-ranged force deﬁned by (3.1) may be transformed into a longer

range force.This mechanism is schematically illustrated in Fig.7.In this ﬁgure the separation of the

interface A is caused by the separation imposed on the two ends of the dashed box,which contains all

motions within the box.Fig.7a is the no sliding case where (3.3) is not satisﬁed;while Fig.7b shows the

case where k

N

is a combination of the normal components of gliding induced separations plus the normal

separation between interfacial atom-pairs.Dislocation motion may thus roughen a fracture surface and,

thereby modify the total surface energy and peak stress.

The mechanism proposed in Fig.7a and b can be stated as the following two hypotheses:

1.The tangential components of dislocation induced sliding trade oﬀ against each other,except the sliding

along the c-plane.

2.If we assume that the change of surface energy is negligible,then the normal components of all sliding

induced separations reduce the peak separation force through rescaling the universal function E

N

.de-

ﬁned in (3.1) in the following manner:

E

N

þj

slide

X

E

S

¼ 2c

F

E

N

j

k

N

k

N0

l

TF

;ð3:12Þ

where j is a re-scaling parameter to be discussed in the following sections.

S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1875

By substituting (3.12) into (3.11),the latter becomes

W

N

¼ 2c

F

E

N

j

k

N

k

N0

l

TF

ð3:13Þ

and

W

T

¼ E

c

:ð3:14Þ

In this paper the eﬀect of dislocation induced atomic vibration (dislocation–phonon interaction) is

omitted.

Fig.7.Normal separation and sliding induced separation:(a) pure normal separation;(b) mixed separation–separation strength

weakens and (c) a dislocation induced sliding may cause a zigzag morphology at fracture surface.

1876 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908

3.5.Grain boundary segregation

An Fe–TiC interface can be viewed as a grain boundary.This is because in practices it is non-trivial to

control all surfaces of a TiC particle to be perfectly coherent to alloy matrix.The vicinity of a grain

boundary interface can be represented by three regions:grain A,grain B,and an interfacial zone h;as

illustrated in Fig.8.Irregularities such as misﬁt in lattice constants,mismatch in atomistic properties and

crystal orientations,molar fraction of the solute,and the free volume in h,may change the energy-sepa-

ration potentials (3.13) and (3.14) signiﬁcantly [25].

According to the thermodynamic description of interfacial segregation,e.g.[26–29],during a fast

fracture at low temperature the reduction of the ideal (Griﬃth) work of separation can be expressed by [27]:

2c

F

¼ 2c

0

F

l

X

I

l

X

S

C

X

;ð3:15Þ

where c

0

F

is the separation energy in a pure system without segregate elements,the superscript ‘‘X’’ denotes

the quantities associated with a segregate element X:C

X

is the quantity of the composition X per unit area

of interface,l

X

I

is the (interfacial) chemical potential of X before separation and l

X

S

is the chemical potential

of the bulk surface phase of X after separation.The value of the quantity ðl

X

I

l

X

S

Þ,where X is one among

the elements of Carbon (C),Phosphorus (P),Tin (Sn),Antimony (Sb),Sulfur (S),are given in [27] based on

experimental data.

Hence,when an interface structure is ﬁxed,the re-scaling parameter j in (3.13) can be computed

accurately.However,it is impractical to do this case by case in engineering design.Accordingly,we

introduce an ad hoc estimate of j for our application.

The idealized coherent interface,e.g.that in Fig.3,can be considered as a degenerate case of Fig.8 when

h ¼ 0 and h ¼ a

i

,where a

i

is the interatomic distance at the interface and it has the same order as the lattice

constants of the matrices.An ad hoc estimate of the re-scaling parameter j in (3.13) is

j ¼

a

i

h

:ð3:16Þ

Alber and Bassani [30] have performed a series of molecular dynamic simulation of the R3 and R5 grain

boundaries.According to the variation of the computed elastic constants their results suggest that h 5a

where a is the lattice constant of A and B in Fig.3 when A¼B.Accordingly,we use a value of j ¼ 1=5 in

this paper,which predicts the maximum separation stress of 6 GPa at the Fe–C site of f001g

Fe

bcc

kf001g

TiC

fcc

interface.This estimate matches experimental results for the commercial steel (modiﬁed 4340 steel) that will

be studied later.This steel shows that the maximum value of ﬂow stress,r

flow

,is near 2 GPa.The slip-line

Fig.8.Schematic diagram of a grain boundary.

S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1877

analysis [23,24] indicates that the maximumseparation stress between a hard inclusion and an iron matrix is

approximately ð1 þ

ﬃﬃﬃ

3

p

Þr

flow

.

Finally,we obtained the normal traction-separations for the Fe–TiC interface which are plotted in Fig.9

using j ¼ 1=5 to calibrate (3.13) based on the results in Fig.4b and Table 1.The curve with the maximum

peak stress is corresponding to the Fe–C site separation while the one with the lowest peak stress is cor-

responding to the Fe–Ti site separation.

4.Quasi-particle dynamics approach

1

As mentioned in Section 2,the secondary particles in ultra high strength steel are on the order of tens

nanometers in size.Materials decohesion and fracture at this scale may depend strongly on atomistic

properties,such as crystal periodicity and orthogonal anisotropy.Molecular dynamics (MD) is an

appropriate method to bridge the quantum physics to continuum mechanical analysis at this scale.

The application of molecular dynamics is hampered by the computational demands of simulating a

suﬃciently large number of atoms to represent the physical phenomenon of interest.The interatomic

distances in a crystal are at the order of Angstroms.Hence,a simulation of a 3D cell model with the

dimension of hundreds nanometers requires about 10

9

atoms.Alaboratory specimen for fracture toughness

is usually on the scale of centimeters.For such a specimen,an ‘‘exact’’ 3D simulation using molecular

dynamics or other atomistic methods requires a model that contains about 10

20

atoms,which is beyond

current computational limits.This motivated the development of the ‘‘Quasi-particle dynamics approach’’;

for short,‘‘Particle Dynamics’’.

The basic idea of ‘‘Quasi-particle dynamics approach’’ is to represent an atomic system as a particle

system through lumping ﬁxed number of atoms into a super-atom,which we call a ‘‘particle’’,while pre-

serving the essential properties of the atomic system via a proposed ‘‘equivalent stiﬀness rule’’.This rule

requires that the particle system has the same crystal structure and stiﬀness coeﬃcients as the original

atomic system but with a larger inter-particle spacing that is determined from the scale of interest,see Fig.

10b and c.The original physics is preserved through transforming the inter-atomic potential (Fig.10a) into

Fig.9.Interfacial metallic debonding/decohesion law.

1

This method is also termed ‘‘Particle Dynamics’’ in other publications of the authors.

1878 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908

an inter-particle potential by preserving the same elastic constants for both systems.More details of the

method can be found in [31].

We reemphasize that the ‘‘particle’’ in ‘‘Quasi-particle dynamics approach’’ is an atomic aggregate and

the number of atoms in the aggregate is determined by the scale of interest.It can represent an inclusion

particle in alloy matrix such as a TiC particle,or just contains a single atom so that the particle system

degenerates to the original crystal.

The ‘‘Quasi-particle dynamics approach’’ is developed based on the two distinct methodologies:The

embedded-atom method (EAM) [32,33] and meshfree methods [34–36].Regarding the literatures of

meshfree methods and other computational methods associated with multi-scale numerical approaches,we

refer to [34,35,37–45].Review of meshfree methods can be found in [46],also recently in [47,48].

Fig.10.Quasi-particle dynamics approach (particle dynamics):(a) conventional Lennard–Jones potential;(b) an atomic system with

the equilibrium interatomic distance a

0

;(c) a particle system with the equilibrium inter-particle distance Na

0

;the particles at this scale

are termed as ‘‘quasi-particles’’;(d) the structural particle system where each structural particle is lumped into several quasi particles;

all structural particles are partitioned into natural elements deﬁned by grain structure and (e) coupling of the continuum mechanics

solution inside a grain with interfacial solution.

S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1879

4.1.Particle system and inter-particle potential

For metals,the EAM [32,33] is a powerful method among those employed in the family of molecular

dynamics.In EAM the total energy E

tot

of a crystal,Figs.3a or 4a,is expressed as the summation of a

combination E

i

for each individual atom:

E

tot

¼

X

i

E

i

;ð4:1Þ

where E

i

is deﬁned by

E

i

¼ F

i

ðq

h

i

Þ þ

1

2

X

i;j;j6

¼i

U

atom

ij

ðr

ij

Þ;ð4:2Þ

where q

h

i

is the total electron density at atom i associated with the host (i.e.,the rest of the atoms in the

system) and F

i

is a function of q

h

i

;U

atom

ij

ðr

ij

Þ is a pair-potential that is the function of the distance r

ij

between

atoms i and j.

We propose an addition term to (4.2)

E

i

¼ F

i

ðq

h

i

Þ þ

1

2

X

i;j;j6

¼i

U

atom

ij

ðr

ij

Þ þ

X

i;j;k;j6

¼k;

j6

¼i;k6

¼i

G

ijk

ðh

ijk

Þ;ð4:3Þ

where G

ijk

ðh

ijk

Þ is the energy associated with rotation,h

ijk

is the angle between bonds i j and i k.

As suggested in [49],the function F

i

ðq

h

i

Þ in (4.2) can be written as

q

h

i

¼

X

j;j6

¼i

r

0

ij

r

ij

"#

6

and q

0

i

¼

X

j;j6

¼i

1 ð4:4aÞ

and

F

i

ðq

h

i

Þ ¼ ðE

sep

E

empty

Þ 1

m

0

Log

q

h

i

q

0

i

q

h

i

q

0

i

m

0

;ð4:4bÞ

where the superscript ‘‘0’’ denotes the variables,e.g.r

ij

¼ r

0

ij

,at equilibriumcondition;m

0

is a constant to be

determined;E

sep

and E

empty

are atomic separation energy and unrelaxed empty site formation energy,

respectively;where the former is deﬁned by (3.2),the latter is obtained from the results listed in Table 1.A

general approach to determine E

i

according to atomic separation (3.1) is given in [50].

We propose the three-body energy term in the form as

G

ijk

ðh

ijk

Þ ¼ c

US

½ðcos h

ijk

cos h

jki

cos h

kij

Þ

m

1

c

3

;ð4:5Þ

where h

ijk

is the angle between r

ij

and r

ik

,r

ij

denotes the vector starting at atomi and ends at atomj;m

1

¼ 1

and c

3

¼ 0:1887 for bcc-Fe crystal.

For the atomic systemshown in Fig.10b,in general,the pair potential U

atom

ij

ðr

ij

Þ can be characterized by

the Lennard–Jones potential (Fig.10a):

U

atom

ij

¼ 4e

0

r

0

r

ij

12

"

r

0

r

ij

6

#

ð4:6Þ

which contains two scaling parameters r

0

and e

0

.The former is the ‘‘collision diameter’’ that refers to the

separation for which the energy is zero;and the latter is the ‘‘depth of the well’’ as demonstrated in Fig.10a.

1880 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908

Thus,the atomic system in Fig.10b is completely deﬁned when its crystal structure is given with a ﬁxed

potential (4.1)–(4.5).Consequently,when the aggregate particle system in Fig.10c has the same crystal

structure as the system in Fig.10b with a similar inter-particle potential like (4.1)–(4.5),then the particle

systemcan be used to reproduce the kinetics and dynamics of the systemin Fig.10b with the accuracy up to

the spacing between the particles.The key-issue here is to ﬁnd the parameters r

0

and e

0

in the inter-particle

potential for the aggregated system so as to preserves the same stiﬀness coeﬃcients of the atomic system.

For a cubic system such as bcc and fcc,the crystal stiﬀness is determined by three independent elastic

constants:C

11

,C

12

,and C

44

[32,33].For a given cubic crystal,the parameters r

0

and e

0

,together with the m

0

in (4.4b) can be ﬁxed by these elastic constants,and vice versa.We use the same concept to develop an

‘‘equivalent stiﬀness rule’’ for the ‘‘Quasi-particle dynamics approach’’,i.e.so that the aggregate particle

system has the same stiﬀness coeﬃcients as the underlying crystal.

In this analysis,Roses relation (3.1) is used to ﬁt (4.4) and (4.6) for an atomic systemlike Fig.10b while

m

0

is set to be 0.36 according to results in [51,52].The system in Fig.10b is partitioned into several sub-

domains and the atoms in each sub-domain are lumped into a single particle,as illustrated in Fig.10c.The

size of each sub-domain is determined by the length scale of interest.The ‘‘equivalent stiﬀness rule’’ is

applied to establish the potential for this ‘‘Quasi-particle dynamics approach’’ system.

For simpliﬁcation,here we consider the case of inﬁnitesimal deformation without relative rotation.

There is no diﬃculty to extend this procedure to the ﬁnite deformation case.For an inﬁnitesimal motion of

an atom i in a crystal characterized by (4.2),the change of the energy DE

i

associated with the atom i is

DE

i

¼ F

i

q

h

i

F

i

q

h0

i

þ

1

2

X

j

U

atom

ij

ðr

ij

Þ

h

U

atom

ij

ðr

0

ij

Þ

i

;ð4:7Þ

where j is summed over all neighbors of i if r

ij

is less than a given cut-oﬀ radius.The term

F

i

ðq

h0

i

Þ þ

1

2

P

j

½U

atom

ij

ðr

0

ij

Þ denotes a reference state and is a constant.The derivation operations of DE

i

with

respect to the distances to neighbor atoms along a given direction reﬂects the stiﬀness of the crystal in this

direction,which is interpreted as an orientation dependent elastic constant [32].When the system is under

pure volumetric,rhombohedral shear,and tetragonal shear deformation,respectively,one can derive the

corresponding bulk modulus K,rhombohedral shear modulus G

1

and tetragonal shear modulus G

2

.This

provides three conditions to calibrate R

0

,E

0

,and M

0

for the EAM-type energy for the Quasi-particle

dynamics approach system in Fig.10c:

E

QP

i

¼ F

i

ðK

h

i

Þ þ

1

2

X

i;j;j6

¼i

U

QP

ij

ðR

ij

Þ ð4:8Þ

through preserving the same K,G

1

and G

2

as that in the underlying crystal.In (4.8) the superscript ‘‘QP’’

refers to quantities in the Quasi-particle system such as in Fig.10c,and

K

h

i

¼

X

j;j6

¼i

R

0

ij

R

ij

"#

6

:ð4:9Þ

For a bcc or fcc crystal,this transformation can be derived analytically according to crystal distortions [53].

In this study,the proposed ‘‘Quasi-particle dynamics approach’’ is applied for two objectors:bcc-Fe matrix

and TiC–Fe interface.In the former the EAMpotential (4.4)–(4.6) are used where m

0

¼ 0:36;for the latter

only the pair potential (4.6) is applied as m

0

is set to be zero.The TiC matrix is considered to be continuum

elasticity.To illustrate we consider the case that m

0

¼ 0 in bulk iron matrix so the ﬁrst termof (4.8) vanishes

and only the calibrations of r

0

and e

0

are required.

Consider a bcc crystal with lattice constants fa

1

;a

2

;a

3

g;at the equilibrium state,a

i

¼ a

0

,for i ¼ 1;2;3.

Any atom in such a bcc crystal has eight neighbor atoms at a distance of r

1

¼ a

0

ﬃﬃﬃ

3

p

=2,six neighbors at a

S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1881

distance of r

2

¼ a

0

,eight neighbor atoms at a distance r

3

¼ a

0

ﬃﬃﬃ

2

p

.In order to illustrate the concept,we cut

oﬀ the ‘‘domain of inﬂuence’’ of the potentials (4.6) to be less than r

3

.

When the crystal is under volumetric deformation

a

1

¼ a

2

¼ a

3

¼ a ð4:10Þ

and the bulk modulus at the position that the atom i occupies is

K

atom

¼

1

9ða

0

Þ

2

½3a

0

ðU

atom

i1

ðr

1

ÞÞ

00

þ3a

0

ðU

atom

i2

ðr

2

ÞÞ

00

4

ﬃﬃﬃ

3

p

ðU

atom

i1

ðr

1

ÞÞ

0

6ðU

atom

i2

ðr

2

ÞÞ

0

;ð4:11Þ

where

ðUðxÞÞ

0

¼

dðUðxÞÞ

dx

and ðU

atom

ij

ðr

j

ÞÞ denotes the potential (4.6) of atom i to the neighbor with the distance r

j

,j ¼ 1;2.For

inﬁnitesimal strain,K

atom

is constant because

ðU

atom

a1

ðr

1

ÞÞ

0

¼ U

atom

a1

a

0

ﬃﬃﬃ

3

p

2

! !

0

;ðU

atom

a2

ðr

2

ÞÞ

0

¼ ðU

atom

a2

ða

0

ÞÞ

0

:

Similarly,when the bcc crystal is under a rhombohedral shear deformation

a

1

¼ a;a

2

¼ a

3

¼ 2a

0

a ð4:12Þ

and the corresponding rhombohedral shear modulus at site i is

G

atom

¼

1

9ða

0

Þ

2

½3a

0

ðU

atom

i1

ðr

1

ÞÞ

00

þ4

ﬃﬃﬃ

3

p

ðU

atom

i1

ðr

1

ÞÞ

0

þ9ðU

atom

i2

ðr

2

ÞÞ

0

:ð4:13Þ

The bcc atomic crystal of Fig.10b is aggregated into a ‘‘bcc quasi-particle crystal’’ with spacing Na

0

in

Fig.10c.This quasi-particle system is characterized by the potential

U

QP

ij

¼ 4E

0

R

0

R

ij

12

"

R

0

R

ij

6

#

;ð4:14Þ

where R

ij

is the distance between a quasi-particles pair i and j.By restricting the domain of inﬂuence of

(4.14) to the ﬁrst two closest neighbor-particles and repeating the procedure (4.10)–(4.13),we obtain

K

QP

¼

1

9ðNa

0

Þ

2

½3Na

0

ðU

QP

ij

ðR

1

ÞÞ

00

þ3Na

0

ðU

QP

ij

ðR

2

ÞÞ

00

4

ﬃﬃﬃ

3

p

ðU

QP

ij

ðR

1

ÞÞ

0

6ðU

QP

ij

ðR

2

ÞÞ

0

ð4:15Þ

and

G

QP

¼

1

9ðNa

0

Þ

2

½3Na

0

ðU

QP

ij

ðR

1

ÞÞ

00

þ4

ﬃﬃﬃ

3

p

ðU

QP

ij

ðR

1

ÞÞ

0

þ9ðU

QP

ij

ðR

2

ÞÞ

0

;ð4:16Þ

where

R

1

¼ Na

0

ﬃﬃﬃ

3

p

2

;R

2

¼ Na

0

:

Now introduce the equivalent stiﬀness rule by setting

K

QP

¼ K

atom

;G

QP

¼ G

atom

:ð4:17Þ

These two equations determine the parameters E

0

and R

0

in the particle potential deﬁned by (4.14).

1882 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908

At the Fe–TiC interface shown in Fig.3a where Fe is bcc and TiC has the (NaCl)fcc crystal structure,we

assume two classes of quasi-particle potentials:the potentials for the bulk Fe or TiC matrix and interfacial

potential.Eqs.(4.10)–(4.17) describe the procedure to obtain the quasi-particle dynamics potential of bulk

bcc-iron crystal.The TiC matrix is presumed pure elasticity.

The proposed ‘‘equivalent stiﬀness rule’’ is also applied for determining the quasi-particle interfacial

potential.The interatomic potential at TiC–Fe interface has already been obtained in Section 3,shown in

Figs.4b and 9.The elastic constant associated with the direction perpendicular to the interface,denoted as

C

Fe–TiC

?

,is calculated by the second order derivative of (3.1) [13]

C

FeTiC

?

¼

2c

F

l

atom

d

2

E

N

dk

2

N

TiC–Fe

;ð4:18Þ

where l

atom

is the interfacial interplanar spacing of the atomic system at equilibrium state,see

Table 1.Using (4.6) to describe (3.1),r

0

an e

0

of (4.6) are determined according to l

atom

and total decohesion

energy.

Assuming that l

QP

,the interfacial interplanar spacing for the quasi-particle dynamics approach systemat

equilibrium state,is given by

l

QP

¼ Nl

atom

;ð4:19Þ

where N is deﬁned in Fig.10c;we have

C

FeTiC

?

¼ l

QP

d

2

U

QP

dR

2

;ð4:20Þ

where U

QP

is the quasi-particle interfacial potential.

By comparing (4.20) with (4.18),together with (4.19),we have two relations to calculate the parameters

in U

QP

deﬁned by (4.14).

4.2.Coupling of quasi-particle dynamics approach and continuum mechanics

Here,we propose a procedure that couples the ‘‘quasi-particle dynamics approach’’ with the continuum

mechanics simulation.

To aﬀect the coupling behavior between the discrete quasi-particle representation and a continuum,a

lumping procedure similar to that employed in quasi-continuum method [54,55] is used.Using meshfree

method,each grain or inclusion particle is discretized into several nodes that are termed ‘‘structural par-

ticles’’.Each structural particle is lumped by several quasi particles,as illustrated in Fig.10d.The quantities

associated with a structural particle I is denoted by the capital subscript I and the quantities associated with

a quasi-particle i is denoted by the plain subscript i.

We assume that the velocity ﬁeld

_

u for the problems in Fig.10d–e can be written as an multi-level

decomposition [38,40,44,56]

_

u ¼

_

u

C

þ

_

u

SP

_

w;ð4:21Þ

where

_

u

C

is the continuum velocity ﬁeld,

_

u

SP

the velocity ﬁeld described by discretized nodes (structural

particles) and

_

w the overlapping velocity ﬁeld bridging continuumand particle scale.For application of this

approach,see [40,44,56–58],also in [59],where a introduction is given to associated with other approaches.

The continuum mechanical solution

_

u

C

is determined through the total Lagrange weak form [60]

Z

X

I

q

C

0

d

_

u

C

þsðu

C

Þ:rd

_

u

C

dX

I

Z

C

I

t

t d

_

u

C

dC

I

t

¼ 0;ð4:22Þ

S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1883

where q

0

is the density at reference conﬁguration and s is the ﬁrst Piola–Kirchhoﬀ stress tensor,X

I

is a

reference domain that coincides to the grain I in Fig.10d and e,C

I

t

is the boundary of X

I

where the traction

t is applied.In a discretized ‘‘structural particle’’ system,the last term in (4.16) is expressed in the form as

Z

C

I

t

t d

_

u

C

dC

I

t

¼

X

N

J

J¼1

w

J

t

J

d

_

u

C

J

;ð4:23Þ

where the subscript ‘‘J’’ denotes the quantities at node J and w

J

is the weight at this node;there are in total

N

J

nodes (structural particles) in X

I

on which the force

t

J

is imposed.The moving particle ﬁnite element

method is applied to solve (4.22) and (4.23) in each X

I

and the interaction between X

I

1

and X

I

2

is governed

by the interfacial potential deﬁned in (4.24) as below.

The solution of (4.22) requires knowledge of a constitutive relation,which can be obtained in two ways:

to deﬁne a structural particle pair potential using the same procedure for quasi particles and to engage a

continuumanalytical model [61] based on the Cauchy–Born law.The second way is applied in this analysis.

The details will be given in the following sections.

The u

SP

is solved using the potential deﬁned below.Let X

I

1

;X

I

2

;X

I

3

...be the domain of the grains

I

1

;I

2

;I

3

;...(the sub-domain of the secondary partitioning in Fig.10d);the pair potential between a

structural particle J

1

in X

I

1

and another structural particle J

2

in X

I

2

is deﬁned as

U

SP

J

1

J

2

¼

P

N

J1

i¼1

P

N

J2

j¼1

U

QP

ij

ðR

ij

Þ for X

I

1

6

¼ X

I

2

;

0 for X

I

1

X

I

2

;

ð4:24Þ

where U

SP

J

1

J

2

is the pair potential in the structural particle system and U

QP

ij

ðR

ij

Þ is the pair potential between

the quasi-particle i that is lumped to the structural particle J

1

and the quasi-particle j is lumped to the

structural particle J

2

;N

J1

and N

J2

denote the number of quasi-particles lumped to J

1

and J

2

,respectively.At

Fe–TiC interface,the U

QP

ij

is determined according to (4.18)–(4.20).

The potential U

SP

J

1

J

2

in (4.24) establishes the bonds between X

I

1

and X

I

2

.Hence,the solution of u

SP

provides the boundary condition of u

C

,as illustrated in Fig.10e.

To trade oﬀ the overlapping between u

SP

and u

C

,the term

_

w in (4.21) is deﬁned as

_

w ¼

_

u

C

at structural node J

1

:U

SP

J

1

J

i

6¼ 0;

0 at structural node J

1

:U

SP

J

1

J

i

0:

(

ð4:25Þ

Thus,the boundary value problem deﬁned in Fig.10e is solved through the continuum mechanics weak

form (4.22) with the boundary conditions deﬁned by (4.23) and (4.24).

5.Hierarchical unit cells and constitutive model

In this section we discuss the response of the sub-micro unit cell and microcell models with secondary

and primary inclusions by employing the ﬁrst principle-based potential obtained in the previous sections.

The procedure summarized in Figs.1 and 2 is engaged in this analysis.The resulting macroscale consti-

tutive law will then be applied in a macroscale simulation of ductile fracture.The experimental results of

modiﬁed 4340 steel [62,63] are used as an example in the simulation.For the constitutive modeling of

heterogeneous system,we refer [64–80].

5.1.A thermodynamic framework for multi-physics computational mechanics

First we establish a thermodynamic framework for computational mechanics analysis based on the

theory of Hughes [81],which provides the necessary conditions for

1884 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908

• setting up a constitutive model without violation of the energy conservation law

• conducting a stabilized numerical simulation.

In the following analysis,we use r to represent the Cauchy stress tensor and

_

the symmetric part of the

velocity gradient.Both the Cauchy stresses and velocity gradient can be at either sub-micro-,micro-,or

macroscale.All analysis will be performed in a co-rotation conﬁguration so the change of stress due to

system rotation is removed.The notations and formulations of continuum plasticity introduced in [60] are

applied in this analysis.The detailed formulation of the co-rotation operation under large deformation is

introduced in Appendix B.

We assume the additive decomposition of strain rate

_

_

¼

_

e

þ

_

p

;ð5:1Þ

where the superscript ‘‘e’’ denotes the elastic part and ‘‘p’’ denotes the plastic part.More explanation about

(5.1) is introduced in Appendix C.

In conventional continuum plasticity

_

r ¼ D

e

:

_

e

;

_

p

¼

_

e

oU

or

;ð5:2Þ

where D

e

is elastic stiﬀness matrix,

_

e is ‘‘ﬂow factor’’,U is the plastic potential to be found

U ¼ Uðr;k

1

;k

2

;...;k

m

Þ;ð5:3Þ

where k

k

are internal variables,such as equivalent plastic strain,damage,etc.

Following the conventional elastic–plastic analysis,e.g.the procedure introduced in [60],(5.7) leads to

the incremental formulation of constitutive law when U is known:

Dr ¼ D

ep

:D

_

;

where

D

ep

¼ D

e

ðD

e

:U

r

ÞðU

r

:D

e

Þ

P

k

h

k

U

k

k

þU

r

:D

e

:U

r

ð5:4Þ

and

U

k

k

¼

oU

ok

k

;U

r

¼

oU

or

;

_

k

k

¼

_

eh

k

¼

_

e

oW

k

oF

k

;

where F

k

,k

k

are conjugate pairs of the internal variables in (5.3) and the corresponding general thermo-

dynamic force,respectively.For example,F

k

,k

k

can be the pair of stress r and strain ,the interfacial

traction

t and separation ½u,a scale damage f and its driving force h,temperature gradient and heat ﬂux,

etc.W

k

is the corresponding energy dissipation of the pair ðF

k

;k

k

Þ

W

k

¼

Z

k

k

0

F

k

dk

k

:ð5:5Þ

We want to ﬁnd the general rule to establish a potential U in (5.2) for a system with multi-physics.

Hughes [81] has proven that the stability of a computation mechanics solution is determined by the sat-

isfaction of the local form of the Clausius–Duhem inequality

X

k

½F

k

_

k

k

_

W

k

ð

_

k

k

;TÞ

_

uð

_

e

;TÞ þs

_

T P0;ð5:6Þ

where T,s,u denote in turn the temperature,entropy,and free energy.The Clausius–Duhem inequality is

actually an alternative representation of the second thermodynamic principle [82],which has been widely

S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1885

applied in the constitutive models,e.g.in [82–84].However,only [81] reveals that (5.6) is equally important

for both constitutive modeling and numerical simulation,which is crucial for computational material de-

sign.

In this analysis we assume no heat supply and conduction.Considering the simplest case in Fig.10e:only

the conjugate pairs of stress–strain ðr;Þ,interfacial traction and separation ð

t;½uÞ,scale damage and its

driving force ðh;f Þ,are taken into account;then (5.6) becomes

r:

_

þt ½

_

u þh

_

f

_

uð

_

e

;TÞ

_

W

t

_

W

f

þs

_

T P0;ð5:7Þ

where W

t

and W

f

are the energy dissipations of ð

t;½uÞ and ðh;f Þ,respectively;and

_

u ¼

ou

o

e

:

_

e

þ

ou

oT

_

T;

_

W

t

¼

oW

t

o½u

:½

_

u þ

oW

t

oT

_

T;

_

W

f

¼

oW

f

of

_

f þ

oW

f

oT

_

T:ð5:8Þ

On the other hand

r ¼

ou

o

e

;s ¼

ou

oT

þ

oW

f

oT

þ

oW

t

oT

:ð5:9Þ

Substituting (5.8) and (5.9) into (5.7),it can be satisﬁed if

t ¼

oW

t

o½u

;h

f

¼

oW

f

of

ð5:10Þ

and

r:ð

_

_

e

Þ P0:ð5:11Þ

The ﬁrst relation in (5.10) requires W

t

to be Needlemans potential,e.g.deﬁned by (4.24).The second

relation of (5.10) deﬁnes a potential of damage.By comparison (5.11) with (5.2),we obtain

_

r:

oU

or

P0:ð5:12Þ

This equation lays down a ‘‘convex condition’’ for any proposed plastic potential U,which also deﬁnes the

local form of stability condition for the multi-physics computational mechanics approach.At a material

point,(5.12) is an alternate expression of Druckers postulate for isotropic plasticity.

5.2.Two-level cell modeling

The cell models for determining the constitutive response are based on periodic distributions of inclusion

particles.Hence,according to the arrangements of the inclusions,three representative cells are illustrated in

Fig.11a.Using periodic and symmetric properties,the three-dimensional cubical primitive distribution can

be simpliﬁed to the two-dimensional rectangular cell with single inclusion;whereas the 3D body central

cubic or hexagonal distribution can be simpliﬁed to the 2D rectangular cell with double inclusions,as

shown in Fig.11b.By varying the shape,size and distributions of the primary/secondary inclusion particles

and the decohesion energies,the methodology of computational cell modeling introduced,e.g.in

[67,69,70,74,85],is applied in this paper.

The Bishop–Hill relations [86]

R

ij

¼

1

V

cell

Z

V

cell

r

cell

ij

dV;

_

E

ij

¼

1

V

cell

Z

V

cell

_

e

cell

ij

dV ð5:13Þ

are employed in the analysis which establishes the relationship between the homogenized average stress/

strain (R

ij

;E

ij

) response and cell stress/strain (r

cell

ij

;e

cell

ij

).The amplitudes and distributions of r

cell

ij

;e

cell

ij

are

1886 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908

determined by parameters such as the material properties of the cell matrix and inclusion,the interfacial

cohesion,the size and geometries of inclusions,and the load imposed on the cell.Both two dimensional and

three dimensional cells are analyzed.

5.2.1.Sub-microcell model

The sub-microcell simulation aims to:

(1) investigating the eﬀects of the secondary inclusion particles (TiC,about 2–300 nm in size) and debond-

ing behavior on the micro-stress–strain response;

(2) establishing the corresponding constitutive model that is applied as the matrix material in a microscale

cell model.

The quasi-particle dynamics approach is applied in the sub-microscale cell model.At the structural

particles level (Fig.10d and e),the entire iron matrix is treated as a grain and the inclusions are to be other

grains.The interfacial decohesion curves shown in Fig.9 are applied for establishing the particle potential

(4.24).The secondary particle,TiC,is treated as isotropic and linear elastic with the Youngs modulus of

600 GPa and a Poisson ratio 0.3.

A crucial part of this simulation is to establish the constitutive law of the iron matrix.According to the

ﬁrst principle calculation,the (1 11) adhesion energy of pure iron is about 5.5 J/M

2

which leads to a peak

decohesion stress around 45 GPa,see Table 1 and Fig.12a.When point defects,e.g.empty sites,exist,the

adhesion energy drops drastically,see Table 1.Using the homogenization procedure,e.g.[61,87],the

Fig.11.The cell model:(a) three classes of periodic distributions of inclusions and (b) boundary conditions imposed in cell modeling.

S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1887

interatomic force separation relation in Fig.12a can be transformed to an non-linear elastic constitutive law

shown in Fig.12c.

On the other hand,the analysis of Section 3 indicates that a bcc-iron is ‘‘intrinsically ductile’’ according

to (3.3) and the model introduced in Fig.5.The corresponding shear traction vs.gliding separation is

shown in Fig.12b.Applying the model illustrated in Fig.7 to the separation of iron matrix,one can ﬁnd

that the gliding induced dislocation has two obvious eﬀects on the corresponding homogenized stress–strain

Fig.12.The constitutive law of iron matrix,from interatomic force-separation relation to conventional plasticity:(a) interatomic

normal traction vs.separation;(b) interatomic shear force vs.gliding;(c) a non-linear elasticity,homogenized based on (a);(d) a stress–

strain response homogenized combining normal separation and gliding,and J

2

plasticity and (e) experimental measurement of the

modiﬁed 4340 steel [62,63].

1888 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908

response:(1) reducing peak stress;(2) increasing the strain at ﬁnal failure,as show in Fig.12d.Fig.12a–d

actually explain how plasticity occurs in real steel.Theoretically speaking,the amplitude of the ‘‘yield

plateau’’ and the value of the ﬁnal failure strain in Fig.12d can be computed accurately using ﬁrst-principle

computation.However,in practice it is diﬃcult to know the exact numbers and positions of point defects

because these parameters actually determine the ﬁnal result.

In this research the iron matrix of sub-microcell is assumed to be a continuum medium governed by

the stress–strain response with a ﬂat ‘‘plateau’’ in Fig.12d.The homogenization of the atomic normal

separation,plotted in Fig.12c,is split into two parts to describe loading stage I and softening stage III

in Fig.12d,respectively;whereas the J

2

plasticity is applied to describe the stage II,i.e.the ‘‘plateau’’.

The experiment result of the modiﬁed 4330 steel [62,63] is applied to calibrate the height of the

‘‘plateau’’ and the onset of softening,denoted as the yield strength r

Y0

and the shear failure strain e

f

,

respectively.

Fig.12e shows the experimental stress–strain curve of the modiﬁed 4340 steel,which is studied in col-

laboration with the Caterpillar Technical Center employing both uniaxial tension and pure shear tests

[62,63].Under the pure shear condition,no signiﬁcant debonding between the primary inclusions and the

alloy matrix has been observed and the material fails entirely by microvoiding at the secondary particles;

therefore the measured initial yield stress is taken as a lower bound whereas the maximum stress is as an

upper bound of the yield strength of the iron matrix since the measured result contains the strengthening

provided by the secondary (TiC) particles after yielding in the steel.

In the computation the initial slope at stage I,which deﬁnes Youngs modulus,is 200 GPa with a Poisson

ratio of 0.3.The r

Y0

,measured at initial yield in the experimental stress–strain curve,is 1.03 GPa and the

failure shear strain is 0.2 according to shear test.

In the sub-microcell modeling,biaxial tension (2D) and triaxial tension (3D) are imposed on the unit cell.

Various ratios of the ﬁrst and the third principle stresses are chosen to reproduce uniaxial tension,pure

shear,and the stress state in-between.The average stresses and strain are measured according to (5.13).

Plotted in Fig.13 are a set of snapshots of the sub-micro equivalent plastic strain contours during

debonding and the corresponding microshear stress–strain response.The cell is under shear dominant

boundary conditions.However,a localized normal separation may also occur.These results demonstrate

that the localization incipience is characterized by onset of the shear bands connecting two inclusions,it

triggers a subsequent fast debonding along the interface and results a sudden drop of the microscale stress.

This phenomenon is quite close to the model and the associated hypotheses in Fig.7,which illustrates that

normal separation is a combination of the normal components of gliding induced dislocation and the

separation between interfacial atom-pairs.For an intrinsically ductile material like bcc-Fe,gliding induced

dislocations motion dominates.Fig.14 shows an experimental observation which demonstrates that a shear

band induces the coalescence of microvoids.

It is well known that parameters such as volume fraction,orientation and distribution of the secondary

particles,as well as stress state and decohesion energy,determine the sub-microcells deformation and

failure behavior.According to the computational results plotted in Fig.13,we conclude that among these

parameters,the decohesion energy is particularly important.Plotted in Fig.15 is a set of computations

where the decohesion energy varies from zero to the upper bound value corresponding to the Fe–C site

conﬁguration (see Fig.3b).In these computations,spacing and volume fraction of the secondary particles

are ﬁxed.If we use the microscale strain E

micro

12

at debonding as a threshold value for the micro-stress–strain

relation,then from Fig.15 we ﬁnd that this debonding strain increases substantially when the decohesion

energy increases.When the decohesion energy reaches its upper bound (3.8 J/m

2

),no debonding takes place

at all.

Fig.16 shows a 3D simulation performed by ﬁnite element method.The cell is under uniaxial tension

with the interfacial decohesion energy 0.6 J/m

2

.This simulation is used to test the model and the parameters

set-up.

S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1889

Based on a large amount of numerical simulation and the methodology of cell modeling introduced in

[88],a general framework of multi-scale constitutive model has been developed,which couples interfacial

debonding,void nucleation and growth,localization with strain gradient eﬀects and phase transformation.

For an isotropic material,the corresponding plastic potential is expressed as

Fig.13.Snap-shots of the localization induced debonding process.

Fig.14.Observation:localization induced decohesion [J.F.Mescall (US Army Mat.Lab)].

1890 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908

U

plasticity

ðf

0

;f;r

ij

Þ ¼

r

r

intr

!

2

þA

0

r

m

r

intr

þA

1

ðf þg

1

Þ exp

r

m

r

intr

þA

2

ðf þg

2

Þ exp

r

m

r

intr

ðq

0

þq

1

ðf Þ

2

Þ ¼ 0;ð5:14Þ

where r

ij

,

r,r

m

f

0

and f denote in turn the stress tensor,equivalent stress,mean stress,inclusion and void

volume fraction at a given scale;r

intr

denotes the ‘‘material intrinsic strength’’ that contains the eﬀects of

internal variables associated with strain softening in post-bifurcation stage;the constants A

i

and q

i

are

calibrated through the cell models.

When the constants A

i

and q

1

in (5.14) vanish,this potential degenerates to the conventional J

2

plasticity

except the yield strength is replaced by ‘‘

ﬃﬃﬃﬃﬃ

q

0

p

r

intr

’’.(5.14) becomes a ‘‘Drucker–Prager-like’’ plastic potential

when A

0

is non-zero whereas convert to a ‘‘Gurson-like’’ model when A

0

¼ 0 but A

1

¼ A

2

and g

1

¼ g

2

¼ 0.

For modiﬁed 4340 steel,the microscale plastic potential is derived

U

micro

ðf

II

0

;f

II

;R

micro

ij

Þ ¼

R

micro

r

flow

!

2

þðf

ðf

II

ÞÞ

g

g

0

expðv

1

Þ

3r

Y0

r

flow

ð1 þðf

ðf

II

ÞÞ

g

qÞ ¼ 0;ð5:15Þ

Fig.15.The eﬀect of decohesion energy on the global stress–strain curves.

Fig.16.Three-dimensional cell modeling.

S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1891

where

R

micro

and R

micro

m

are the equivalent and mean stress of R

micro

ij

,respectively;f

II

0

is the volume fraction of

the secondary particles,f

II

is the volume fraction of the voids nucleated from f

II

0

,f

ðf

II

Þ is the damage

evolution function deﬁned by Tvergaard [89]

f

ðf

II

Þ ¼

0 f

II

< f

II

0

f

II

f

II

0

6f

II

< f

II

c

f

II

c

þK

II

ðf

II

f

II

c

Þ f

II

Pf

II

c

8

>

<

>

:

ð5:16Þ

and the v

1

in (5.15) are the functions deﬁned as

v

1

¼ a

1

f

R

micro

m

R

c

max

r

Y0

þa

2

f

R

micro

R

US

max

r

Y0

!

;ð5:17Þ

where R

micro

m

is the mean stress of R

micro

ij

;a

1

and a

2

are constants,a

1

¼ 1:06,a

2

¼ 0:3.R

c

max

is the strength

against the normal separation of the interface between alloy matrix and secondary particles,i.e.,the peak

stress in traction–separation law in Fig.10.R

US

max

is the shear strength against gliding induced dislocation.

The function f in (5.17) is deﬁned as follows:

fðxÞ ¼

x if x P0;

0 otherwise:

ð5:18Þ

The constants in (5.15)–(5.18) are listed in Table 2.

5.2.2.Microcell model

The constitutive model (5.15) is embedded into the matrix of the cell that contains a primary particle

with a size of around 1–2 lm,as plotted in Fig.17a.This representative unit cell is used to obtain the

macroscale stress–strain relation (R

ij

;E

ij

).In high strength steel,e.g.the modiﬁed 4340 [62,63],the primary

particles are typically titanium nitrides (TiN) of cubical shape,represented in the model as square,see Fig.

17a.

Experimental research reveals that the debonding–decohesion between large nitrides and matrix usually

takes place under relative low load level.This is because the accumulation of misﬁt strain and the segregate

impurity elements (mainly the Sulfur) precipitated along the grain boundary can reduce the interfacial

strength signiﬁcantly.The traction-separation in Fig.9,calibrated according to the peak value given in [63],

is applied in simulation.A typical debonding-localization phenomenon for this class of cell and the cor-

respond slip-ﬁeld are illustrated in Fig.17c.The TiN is assumed to be elastic with a Youngs modulus of

350 GPa [20] and a Poisson ratio of 0.3.

Plotted in Fig.18 are set of computed macroscale stress–strain curves with varying primary inclusion

volume fraction,where the macroscale stress–strain response demonstrates three stages of the cell behavior:

(I) elastic deformation and yielding;(II) debonding/decohesion between large nitride inclusions and the

alloy matrix;(III) post-bifurcation/softening.In contrast to Fig.15,two stress drops appear in stage II.

These are caused by debonding at two perpendicular surfaces of the square nitrides.By varying the shape,

size and distribution of the primary/secondary particles and the decohesion energies,the shape of the

stress–strain curve and positions of the turning-points between diﬀerent stages vary.These provide the

Table 2

Parameters in (5.15)

g

0

g q a

1

a

2

f

II

c

K

II

1.5 2 )0.33333 1.06 0.2 0.05 3

1892 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908

possibility of choosing an optimum combination of particle size,geometry and distribution for micro-

structural design.

The stress and strain at the onset of stage III,as well as the slope of the subsequent softening,are key

parameters linked to the failure behavior of the material.A challenge is how to implement the phenomena

reﬂected in Fig.17 into an applicable constitutive law.We discuss this issue in the following section.

5.2.3.Coupling and macroscale constitutive law

To obtain desirable fracture toughness,the stress–strain response after the onset of softening plays a

signiﬁcant role in crack growth simulation,which actually reﬂects the ﬁnal stage of the coalescence of voids.

In the framework proposed in this paper,a concurrent model is introduced and described as follows.

Fig.17.Microscale cell modeling:(a) TiN [1];(b) microscale cell and (c) localization induced decohesion.

S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1893

Material resistance against void coalescence is determined by the strength of the ligaments between these

voids [88,90].The deformation tolerance and the failure of the matrix ligament are determined by two basic

deformation modes:localization induced necking under normal stress and shear localization caused by the

shear stress component.Consequently,we postulate that the matrix can be divided into two parallel groups

of microscopic elements.The ﬁrst group can be considered as a virtual bond network built in the alloy

matrix;the second group is assumed to be a superposition of imaginary microslices that correspond to the

slip systems along diﬀerent orientations (see Fig.19a–b).In each bond or slice,the strain gradient theory

[91,92]-based 1D localization solutions for tension or pure shear [56] are applied.In this class of solution

the material intrinsic length scale l [91,92] is included and the eﬀects of geometrically necessary dislocations

are taken into account.For isotropic materials,a multi-dimensional stress–strain behavior can be char-

acterized through uniaxial and pure shear strain gradient theory-based solutions,which is represented by

the material intrinsic strength r

intr

presented in (5.14).It provides the matrix material properties after the

onset of strain softening in the microscale cell model (see Fig.19c),in conjunction with primary particles

and the subsequent damage evolution.

Based on the concurrent model and numerical results,by rewriting (5.14) at this scale we obtain a

macroscopic plastic potential

U

macro

¼

R

r

intr

2

þA

0

R

m

r

intr

þA

1

ðf

I

þg

1

Þ exp

R

m

r

intr

þA

2

ðf

I

þg

2

Þ exp

R

m

r

intr

ðq

0

þq

1

ðf

I

Þ

2

Þ ¼ 0 ð5:19Þ

and the associated ﬂow law

_

E

p

¼

_

k

oU

macro

oR

;

where

_

k is the ‘‘ﬂow factor’’,

R and R

m

denote the Cauchy equivalent stress and Cauchy mean stress,

respectively;f

I

represents the void volume fraction which is considered as ‘‘damage’’;A

0

,A

1

,A

2

,g

1

,g

2

,q

0

and q

1

are dimensionless material constants listed in Table 3.The evolution laws of damage nucleation and

growth introduced in [93] and the material parameters of the modiﬁed 4340 steel presented in [63] are

applied in this work.

Fig.18.Macroscale stress–strain response with varying volume fracture of nitrides.

1894 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908

The plastic potential (5.19) is a macroscale,J

2

-like plasticity with damage.The concurrent model

associated with the mechanisms in Figs.18 and 19 is described by ‘‘r

intr

’’ in (5.19),which is termed

‘‘material intrinsic strength’’.It is deﬁned as the combination of a material strain hardening/softening law

and the strain gradient-based traction–separation law:

r

intr

¼

r

Y0

ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ

r

hom

ð

E

p

Þ

r

Y0

h i

2

þlg

r

strain hardening=softening

E

p

6½

E

bifurc

;

Tð

e

Y;l;gÞ decohesion softening

E

p

> ½

E

bifurc

;

8

<

:

ð5:20Þ

where

E

p

is the plastic part of the equivalent strain and ½

E

bifurc

denotes

E

p

at the bifurcation point of the

r

intr

ð

E

p

Þ relation.Originally l is deﬁned as the material intrinsic length scale deﬁned as the product of

Burgers vector b and the initial yield strength r

Y0

;g is the equivalent strain gradient [92]:

Fig.19.Two microscopic elements:virtual bond and shear slice.

Table 3

Parameters in (5.19)

A

0

A

1

A

2

g

1

g

2

q

1

q

0

0.0666 0.85 1.7 0.01 0.01 2.65 1.0255

S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1895

l ¼ 3

E

r

Y0

2

b;g ¼

ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ

1

2

u

k;ij

u

k;ij

r

;ð5:21Þ

where E is Youngs modulus;and the strain-like parameter

e

Y is deﬁned by

e

Y ¼ ð

E

p

½

E

bifur

Þ

l

l

0

;ð5:22Þ

where l

0

is a material constant,of the same order as the spacing between primary particles.½

E

bifurc

marks

the transition between the two stages of deformation:the uniformdeformation with damage nucleation and

growth and the failure of the ligaments between these defects.½

E

bifurc

can be calibrated to the maximum

stress on the r

intr

ð

E

p

Þ curve fromthe uniaxial tension test.During the second stage,the eﬀect of the material

intrinsic length scale,strain gradient,and strain rate are incorporated in r

intr

as

T ¼ r

Y0

e

T ð

E

p

;l;l

0

Þ

ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ

r

hom

ð

E

p

Þ

r

Y0

2

þlg

s

:ð5:23Þ

The second termin (5.23) is the traction–separation law derived fromthe strain gradient-based localization

solution at the microscale;the third and fourth terms reﬂect,in turn,the strain rate eﬀect and the material

hardening due to the strain gradient at macroscale.As the microscale localization,representing ligament

failure,is described by

e

T in (5.23),the stress–strain response without bifurcation,denoted by r

hom

ð

E

p

Þ,

appears under the square root of the fourth term.

Based on the analytical solution described in [88],a ﬁtted expression of

e

T can be expressed as

e

T ¼

0:5398Y

2

þ1:5867Y 0:0466

1 k

tr

;ð5:24Þ

where

Y ¼ exp 10

6

ð

e

Y Þ

11=5

n o

;k

tr

¼

r

I

3r

m

2r

I

and k

tr

< 1:

According (5.1) and (5.2),the plastic part of macroscale strain is determined by the potential (5.19) and

elastic part is determined by Hooks law.As the iron matrix and inclusion particles have diﬀerent Youngs

modulus,a formula to estimate macroscale Youngs modulus is suggested in the form as

E

macro

¼ v

Fe

E

Fe

þv

TiC

E

TiC

þv

TiN

E

TiN

;ð5:25Þ

where ‘‘v

X

’’ denotes the volume fraction of X and E

X

is the Youngs modulus of X.For all components a

Poissons ratio of 0.3 is applied.

6.Laboratory specimen scale:Simulation,results,and discussion

6.1.Fracture toughness simulation

In this section we describe ductile fracture simulation carried out on a center cracked panel according to

the ASTM Standard E399-E1737,which has been applied in the simulations in [85,95],using the hierar-

chical constitutive model developed in the previous sections and the meshfree code [34,35,96].As discussed

in [72,95],the loading speed and materials strain rate sensitivity may have a strong eﬀect on damage

evolution,thus,fracture toughness.However,in this paper only the results under quasi-static loading are

presented.

1896 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908

Fig.20 presents two snapshots of 3Dcrack propagation using the macroscale plastic potential described

in (5.19).Fig.21a shows the contours of equivalent plastic strain around a blunted crack tip at small-scale

yielding,where the Rice-Johnson type crack tip strain ﬁeld is present.Fig.21b shows the contours after

considerable crack growth with large deformation.In this computation the primary particles (TiN) are

explicitly embedded into the matrix that includes the secondary particles so that the microscale plastic

potential (5.14),in conjunction with the (4.24) in quasi-particle dynamics approach,is applied.Plotted in

Fig.21c is the corresponding load–CTOD curve,where a black square indicates the CTOD at crack ini-

tiation which deﬁnes the fracture toughness of the material.Figs.20 and 21 demonstrates that the com-

putational approach is capable of capturing this class of phenomenon.On the other hand,it also reveals

that the computational results depend upon many factors such as the geometry and distribution of

inclusions,which are not readily captured by the periodic cell models in Fig.11.

6.2.Ductile fracture simulator and toughness-strength-adhesion diagram

The hierarchical constitutive and computational methodology introduced in this paper results in a

‘‘ductile fracture simulator’’,illustrated in Fig.22.Starting from the left-lower corner,the quantum

mechanics analysis explores the fundamental atomistic–electronic structures of the alloy matrix and the

matrix/inclusion interface.This provides the corresponding energy–adhesion relations that are applied in

the sub-micro and microcell modeling to obtain the corresponding constitutive relations (5.14),(5.15),

(5.19) for the matrix material in each scale.For the modiﬁed 4340 steel,the computational results have been

calibrated by experiments.The constitutive law (5.19) of a inclusion induced voiding/microvoiding steel is

implemented into compute codes for calculating crack parameters such as the crack tip opening dis-

placement (COD,see Fig.21a) and the J-integral using the method introduced in [97,98].The COD (or

J-integral) at crack growth initiation represents the fracture toughness of the material according to the

ASTM standard.The simulated results are summarized by the toughness–strength–adhesion (TSA) dia-

gram that is at the right-upper corner of Fig.22,which provides insight into the correlations between the

steel strength,interfacial decohesion,and fracture toughness.

The TSAdiagramat the right-upper corner of Fig.22 is detailed in Fig.23.In Fig.23a the ﬁrst principle-

based traction–separation relations are plotted at various adhesion energy levels.Obviously higher

Fig.20.The strain gradient theory-based strain softening solution for the microscopic elements in Fig.19,where l denotes the

microscale length [92] that scales the dissipation during post-bifurcation deformation [56] and l

0

denotes the average spacing between

primary particles.

S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1897

adhesion energy results in higher peak decohesion stress.Fig.23b is the TSA diagramcorresponding to the

TSA curves presented in Fig.23a.

In the TSA diagram(Fig.23b) the dashed lines represent the computed load–COD curves for the center

cracked panel under tension.Simulations with values of matrix yield strengths of 500,700,900 and 1030

MPa are performed using the proposed hierarchical multi-physics constitutive models (5.14),(5.15) and

(5.19).Along each dashed line the circle,delta,solid circle,and triangle denote in turn the CODi (the COD

at crack growth initiation),corresponding to the diﬀerent levels of decohesion energy of the interface be-

tween the iron matrix and the inclusion particles,illustrated in Fig.23a.The solid lines indicate the vari-

ation of fracture toughness when the decohesion energy is ﬁxed but the strength of the iron matrix is varied.

For example,at the decohesion energy of 0.6 J/m

2

,the most right circle denotes the CODat crack initiation

for the matrix with the yield strength of 1.1 GPa.Similarly,the most left circle on the line with 0.6 J/m

2

denotes the COD at crack initiation for the steel with the matrix yield strength 0.5 GPa.

In the simulations presented in the TSAdiagramthe diameters of the primary TiNparticles ranged from

1 to 2 lm with a volume fraction from 0.02% to 0.2%;the diameters of the secondary particles are from 20

to 200 nm with a volume fraction from 0.02% to 0.4%.The computation shows that crack propagation is

mainly governed by the decohesion–debonding process of the primary TiN particles (inclusions) whereas a

uniformly distributed small inclusion particles have a relatively stronger eﬀect on strengthening,rather than

on fracture.More detailed investigations,especially for the system with non-uniformly distributed inclu-

sions,are required for clarifying the dual eﬀects of secondary particles on strengthening and toughness.

Fig.21.A simulation of crack growth:contours of equivalent stress and load–CTOD curve.

1898 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908

Fig.23b reveals that increasing adhesion energy is a way to improve fracture toughness while main-

taining strength.However,the TSA diagram also indicates that the toughening eﬀect of adhesion energy is

relatively reduced at high strength.Apparently,ﬁxing interfacial strength but varying alloy matrix strength

or verse versa may have a similar eﬀect on fracture toughness.The trend obtained from the TSA diagram

coincides with several experimental reports,e.g.[24,99–102].

The TSA diagram in Fig.23b,in conjunction with the analyses presented in the previous sections,

provides several guidelines for steel design:

(1) Both interfacial adhesion energy and strength ratio are crucial for obtaining high toughness with high

strength.A quantitative description of these relationships is given in Fig.23.

(2) Large inclusions (>1 lm) can not maintain high interfacial strength and is the major cause of lower

toughness.

(3) For smaller dispersed particles,dispersion spatial uniformly may be particular important for enhanced

toughness.

(4) The densities of point defects in an alloy matrix,such as vacancies,dislocations,have strong ef-

fects on the strength and fracture mode of the alloy.The ratio between the normal separation

energy and the energy barrier against dislocation motion determines the macroscale strength of

alloys.

Fig.22.Ductile fracture simulator.

S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1899

7.Conclusions

• At atomistic scale the failure of metal can be caused by two diﬀerent mechanisms:normal separation

between atomic pairs and gliding induced dislocation.Rices criterion of ductile-brittle fracture transi-

tion has been applied to determine which of them will occur.

• The density functional theory-based quantum mechanical computation indicates that in bcc-iron crystal

the gliding induced separation is dominant,which explains why plastic ﬂow takes place.

• A ‘‘quasi-particle dynamics approach’’ approach has been developed and is applied at the scale bridging

quantum physics and continuum mechanics.

• A computational thermodynamic framework of metal plasticity,which unions diﬀerent physics concur-

rently,has been developed based on Clausius–Duhem inequality and Hughes stability theory.

• Using a two-level cell modeling,a hierarchical constitutive model has been developed for the ultra-high

strength steels that contain the primary inclusion particles about microns in size and the secondary inclu-

sion particles about 10 nm in size.

• The simulation of ASTMstandard fracture toughness specimen,at ﬁrst time,leads to a multi-scale com-

putation-based TSA diagram,which provides a guideline to assist future alloy design.

• The multi-scale computation indicates that the densities of point defects in alloy matrix have strong ef-

fects on the strength and fracture mode of the alloy.The ratio between the normal separation energy and

the energy barrier against dislocation motion determines the macroscale strength of alloys.

Acknowledgements

The steel design project is funded by ONR (Grant Number:N00014-01-1-0953).Su Hao is funded by

ONR (1/2003-7/2003) and by NSF (3/2002-12/2002).The support of ONR and NSF are greatly appre-

ciated.Su Hao thanks Dr.Singh of NRL for providing the DOD Plane Wave Code and Dr.Mehl of

NRL for providing the NRL Tight-Binding Code.Su Hao is also grateful for the discussions with Prof.

Freeman and Dr.Shishido of Northwestern University,and with Ms.Hsieh and Dr.Sherman of Cater-

pillar Inc.

Fig.23.Toughness–strength-adhesion (TSA) diagram for steel design:(a) interfacial traction–separation relations with various dec-

ohesion energy and (b) TSA diagram where CODi refers the COD at crack initiation.

1900 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908

Appendix A.Preliminary of quantum mechanics and density functional theory [5,6,8,12]

Classical physics views an atom as a nuclei at ﬁxed point surrounded by moving electrons along ﬁxed

orbits.The momentums and positions of nuclei and electrons can be determined exactly according to

Newtons laws.

Quantum mechanics explains nature phenomena through another philosophy.The De Broglie

hypothesis ascribes a wave property to particles such as nuclei and electrons.The Heisenberg uncertainty

principle puts forth that,when the momentumof a particle is known precisely,the position of the particle is

completely unknown.The state of such a particle is deﬁned by Hamiltonian

b

H,the operator corresponding

to the energy of a particle with mass m

b

H ¼

h

2

2m

r

2

þV ðrÞ;ðA:1Þ

where r is the position vector and V ðrÞ is a potential ﬁeld.The eigenvalue equation for

b

H:

b

Hu

i

ðrÞ ¼ E

i

u

i

ðrÞ ðA:2Þ

is called the time-independent Schr

€

odingers equation;where E

i

is the ith eigenvalue and u

i

ðrÞ the ith

eigenfunction.Under this state the expectation to ﬁnd the particle at position x is

hxi ¼

Z

1

1

ru

i

ðrÞ u

i

ðrÞd

3

r ¼

Z

1

1

rju

i

ðrÞj

2

d

3

r:ðA:3Þ

For a many body system,it is usually very diﬃcult to get analytical solution of (A.2) because the po-

tential V ðrÞ is dependent of the interaction among particles.

Thomas–Fermi model approximates the systemas a combination of static atoms which formcrystal and

electronic gas which is ﬁlled in-between.The Hohenberg–Kohn [5] and Kohn–Sham [6] theory states that

the total energy E

total

of a system depends only on the electron density of its ground state

E

total

¼ E

total

ðqðrÞ;R

a

Þ;ðA:4Þ

where R

a

are the position of all atoms in the system under consideration;the electron density q is a scale

function deﬁned as

qðrÞ ¼

X

i

ju

i

ðrÞj

2

:ðA:5Þ

The Hohenberg–Kohn–Sham theorem,the central theorem of the density functional theory,states that

the total system energy gets its minimum value for the ground-state density,denoted as q

0

,and that the

total energy is stationary with respect to its ﬁrst order variations in the density,i.e.:

dE

total

½q

dq

q¼q

0

¼ 0:ðA:6Þ

By varying E

total

with respect to each wave function,it leads to the Kohn–Shams equation:

Hw

i

ðrÞ ¼ e

i

w

i

ðrÞ;H ¼

h

2

2m

r

2

þV

eff

ðrÞ;ðA:7Þ

where w

i

ðrÞ,the solution of Kohn–Shams equation,form an orthonormal set;and the eﬀective potential is

V

eff

ðrÞ ¼ V

C

ðrÞ þl

XC

ðqÞ:ðA:8Þ

Here V

C

ðrÞ is the Coulomb potential;for a condensed system like metal V

C

ðrÞ can be solved through

Poissons equation

S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1901

r

2

V

C

ðrÞ ¼ 4pe

2

qðrÞ;ðA:9Þ

where the qðrÞ denotes the positive point charges of nuclei at its position R

a

and the electronic charge

density qðrÞ in the rest

qðrÞ ¼

Z

r

at R

a

;

qðrÞ otherwise:

The exchange-correlation potential l

XC

ðqÞ is related to the exchange-correlation energy that can not

solved directly in the same way as V

C

ðrÞ.Under the ‘‘local density approximation’’ (LDA) the explicit form

of l

XC

ðqÞ has been derived,e.g.in [103,104]

l

XC

ðqÞ ¼ 2

3q

p

1=3

0:0225Log 1

þ21

4pq

3

1=3

!

:ðA:10Þ

One way to solve (A.7) is to expand the unknown wave function solutions w

i

ðrÞ as a linear combination

of a set of known function with unknown coeﬃcients c

ij

w

i

ðrÞ ¼

X

j

c

ij

/

i

ðrÞ:ðA:11Þ

Substituting (A.11) into (A.7) leads to the following matrix problem:

½

HS c ¼ 0;ðA:12Þ

where

H is the Hamiltonian matrix and S is the overlap matrix

½

H

ij

¼

Z

/

i

H /

j

dr;½S

ij

¼

Z

/

i

/

j

dr ðA:12aÞ

in the ﬁrst relation of (A.12a) the H is deﬁned by (A.7).

The solution procedure is illustrated in Fig.24.

In a periodic structure such as a crystal,according to Bloch theorem the wave function solution w

i

depends upon both position vector r and the reciprocal vector k

w

i

ðr þmG;kÞ ¼ e

ikG

w

i

ðr;kÞ;ðA:13Þ

where G is the primitive vector of the lattice and m is an integer.The corresponding electron density yields

the integration over the ﬁrst Brillouin zone:

qðrÞ ¼

Z

1

st

BZ

#½E

F

e

i

ðkÞjw

i

ðr;kÞj

2

dk;ðA:14Þ

where the step function#insures that only occupied states below the Fermi energy E

F

are counted.

Appendix B.Co-rotational formulation in ﬁnite deformation

The co-rotational formulation introduced in [60,105] is applied in the analysis presented in this work.We

use bold-faced x to represent the coordinate of a material point in a reference coordinate system,i.e.the

Lagrange conﬁguration;and bold-faced y to represents the coordinate of a point in the spatial (Euler)

coordinate system.Obviously

y ¼ yðx;tÞ:ðB:1Þ

1902 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908

Consider a line element vector dr

0

in the reference conﬁguration,after deformation it becomes the line

element dr in the spatial conﬁguration.The deformation gradient is deﬁned by

Fðx;tÞ ¼

oy

ox

;ðB:2Þ

which uniquely determines the line element transformation between the two conﬁgurations

dr ¼ Fdr

0

:ðB:3Þ

Using this relation we can also derive the transformation an area or a volume between two conﬁgura-

tions.When we assume ﬁnite deformation without diﬀusion,then F is non-singular and can be decomposed

multiplicatively as the product of two other positive deﬁnite tensors

F ¼ R

F

U

F

;ðB:4Þ

where R

F

is the orthogonal,positive deﬁnite,tensor of pure rotation from conﬁguration x to y;U

F

is the

positive deﬁnite tensor of pure stretch during deformation.The discussions of the transformations (B.1)–

(B.4) in crystal plasticity and atomistic simulation can be found in [106–108].

The material derivative of Eq.(B.2) leads to

_

Fðx;tÞ ¼

o

_

y

oy

oy

ox

¼ L F with L¼

def

o

_

y

oy

¼ rv:ðB:5Þ

Here we adopt r to represent the gradient operator in the spatial conﬁguration and v ¼

_

y,i.e.the velocity.

So L is called the ‘‘velocity gradient’’.L and Cauchy stress r build a conjugate energy pair.In general,the

rate constitutive relation of a material can be written as

_

r ¼ C:L þS:L

skew

;ðB:6Þ

where C is a material tangent matrix and L

skew

represents the skew-symmetric part of L.The product

S L

skew

reﬂects the change of stress state due to rigid rotations,therefore Eq.(B.6) is ‘‘non-objective’’.

Fig.24.Flow chart of the solution procedure of DFT.

S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1903

In numerical analysis,when a body deforms from step n to step n þ1,its spatial coordinate y

nþ1

may be

written as a function of the conﬁguration at step n and the step length Dt

y

nþ1

¼ y

nþ1

ðy

n

;DtÞ ðB:7Þ

The displacement increment of this point over the step is

Du ¼ y

nþ1

y

n

:ðB:8Þ

An incremental form of the velocity gradient deﬁned in Eq.(B.5) is

L ¼

1

Dt

oDu

oy

nþ1

:ðB:9Þ

The key idea of the co-rotational formulation is to split one increment into two steps,i.e.rotation and

pure deformation.Consider the conﬁguration at y

n

as the reference conﬁguration

_

Fðy

n

;tÞ ¼

_

F

def

ðy

n

;tÞ

_

F

rot

ðy

n

;tÞ:ðB:10Þ

From Eq.(B.4) it is known that

_

F

rot

ðy

n

;tÞ ¼ R I and

_

F

def

ðy

n

;tÞ ¼

oy

nþ1

oy

n

L

def

¼ I

þ

oDu

def

oy

n

oDu

def

Dtoy

nþ1

;ðB:11Þ

where R deﬁnes the rotation from conﬁguration y

n

to y

nþ1

and I represents the unit tensor.If Du

def

is small

enough,then the second relation in Eqs.(B.11) becomes

_

F

def

ðy

n

;tÞ ¼ I L

def

þoðL

def

Þ:ðB:12Þ

The corresponding algorithm for integrating the constitutive equation is as follows:

^

r

nþ1

¼ R

T

r

n

R;

Dr ¼ C:ðDtL

def

Þ;

r

nþ1

¼

^

r

nþ1

þDr:

ðB:13Þ

The second relation in Eqs.(B.13) is ‘‘objective’’ since there is no rotation.

A concise way to calculate R is given in [105] when the rotation is less than p during Dt.Consider a mid-

deformation conﬁguration:

y

nþa

¼ ð1 aÞy

nþ1

þay

n

with 0 < a < 1 ðB:14Þ

it has been proven,elsewhere,that

R ¼ 1

þ

1

2

x

1

1

2

x

1

;g ¼

oDu

oy

nþa

;x ¼

1

2

ðg g

T

Þ;ðB:15Þ

where I is unit tensor.a ¼ 0:5 is used in the analysis.

The formulation listed above can be applied in both Lagrange conﬁguration-based and Euler conﬁgu-

ration-based computation.When a Lagrange conﬁguration is applied,the corresponding derivative oper-

ations are derived in the reference conﬁguration x while the velocity is deﬁned with respect to the current

conﬁguration y

nþ1

,a transformation matrix J is necessary for deﬁning the large strain-velocity matrix

e

B.

o

oy

nþ1

¼

o

ox

ox

oy

nþ1

¼

o

ox

J:ðB:16Þ

Because of

ox

ox

¼

ox

oy

nþ1

oy

nþ1

ox

¼ I:ðB:17Þ

1904 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908

Thus,we have

J ¼

oy

nþ1

ox

1

:ðB:18Þ

Appendix C.The approximation of additive decomposition (5.1)

In a co-rotation coordinate system introduced in Appendix B,the rotation part is removed and the

deformation can be divided into two steps:pure elastic transformation F

e

and plastic transformation F

p

[109]

F ¼ F

p

F

e

Following the procedure giving in [60],the velocity gradient L of the deformation ﬁeld (B.1),deﬁned as

the mass derivative of F,is

L ¼

DF

Dt

¼

oF

ot

F

1

¼

_

F F

1

;ðC:1Þ

which has two parts

_

F F

1

¼

_

F

e

F

p

ðF

e

F

p

Þ

1

þF

e

_

F

p

ðF

e

F

p

Þ

1

¼

_

F

e

ðF

e

Þ

1

þF

e

_

F

p

ðF

p

Þ

1

ðF

e

Þ

1

ðC:2Þ

In this paper,we assume that elastic deformation is inﬁnitesimal so that

F

e

¼ I þ

ou

e

ox

¼ I þoðIÞ;ðF

e

Þ

1

¼ I oðIÞ

and

L ¼

_

F F

1

ﬃ

_

F

e

ðF

e

Þ

1

þ

_

F

p

ðF

p

Þ

1

Deﬁne strain rate as the symmetrical part of the velocity gradient

_

¼ symðLÞ:

We obtain the additive decomposition of strain rate

_

:

_

¼

_

e

þ

_

p

;ð5:1Þ

where

_

e

¼ symð

_

F

e

ðF

e

Þ

1

Þ;

_

p

¼ symð

_

F

p

ðF

p

Þ

1

Þ:

References

[1] Cybersteel2020,ONR contract grant number:N00014-01-1-0953;PIs:Olson GB,Freeman A,Liu WK,Moran B,Northwestern

University.

[2] J.R.Rice,Dislocation nucleation from a crack tip––an analysis based on the Peierls concept,J.Mech.Phys.Solids 40 (2) (1992)

239–271.

[3] L.H.Thomas,The calculation of atomic ﬁelds,Proc.Camb.Philos.Soc.23 (1927) 542–548.

[4] E.Fermi,A statistical method for the determination of some atomic properties and the application of this method to the theory

of the periodic system of elements,Z.Phys.48 (1928) 73–79.

[5] P.Hohenberg,W.Kohn,Inhomogeneous electron gas,Phys.Rev.136 (3B) (1964) 864–871.

[6] W.Kohn,L.J.Sham,Self-consistent equations including exchange and correlation eﬀects,Phys.Rev.140 (4A) (1965) 1133–1138.

S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1905

[7] J.C.Slater,Wave functions in a periodic potential,Phys.Rev.51 (1937) 846–851.

[8] H.Krakauer,A.J.Freeman,Linearized augmented plane-wave method for the electronic band-structure of thin-ﬁlms,Phys.Rev.

B 19 (4) (1979) 1706–1719.

[9] NRL,DoD plane wave:a general scalable density functional code,2002.

[10] M.J.Mehl,D.A.Papaconstantopoulos,Applications of a tight-binding total-energy method for transition and noble metals:

elastic constants,vacancies,and surfaces of monatomic metals,Phys.Rev.B 54 (7) (1996) 4519–4530.

[11] D.A.Papaconstantopoulos,M.J.Mehl,The tight-binding method for interpolating ﬁrst-principles total energy results,J.Phase

Equilib.18 (6) (1997) 593–597.

[12] E.Wimmer et al.,Full-potential self-consistent linearized-augmented-plane-wave method for calculating the electronic-structure

of molecules and surfaces––O

2

molecule,Phys.Rev.B 24 (2) (1981) 864–875.

[13] J.H.Rose,J.R.Smith,J.Ferrante,Universal features of bonding in metals,Phys.Rev.B 28 (4) (1983) 1835–1845.

[14] J.Weertman,Crack tip blunting by dislocation pair creation and separation,Philos.Mag.A––Phys.Cond.Matter Struct.

Defects Mech.Prop.43 (5) (1981) 1103–1123.

[15] S.H.Jhi,J.Ihm,S.G.Louie,M.L.Cohen,Electronic mechanism of hardness enhancement in transition-metal carbonitrides,

Nature 399 (6732) (1999) 132–134.

[16] T.Shishidou et al.,Overlayer and superlattice studies of metal/ceramic interfaces:Fe/TiC,J.Appl.Phys.93 (10) (2003) 6876–

6878.

[17] T.Shishidou,Y.J.Zhao,A.J.Freeman,private discussion,2002.

[18] M.J.S.Spencer et al.,Further studies of iron adhesion:(11 1) surface,Surf.Sci.515 (2002) L464–468.

[19] M.J.Mehl,A.Papaconstantopoulos,Application of a tight-binding total-energy method for transition and noble metals:elastic

constants,vacancies,and surfaces of monatomic metals,Phys.Rev.B 54 (7) (1996) 4519–4530.

[20] S.H.Jhi,J.Ihm,Electronic structure and structural stability of TiC

x

N

1x

alloys,Phys.Rev.B 56 (21) (1997) 13826–13829.

[21] A.J.Freeman,Materials by design and the exciting role of quantum computation/simulation,J.Computat.Appl.Math.149 (1)

(2002) 27–56.

[22] D.G.Pettifor,A.H.Cottrell (Eds.),Electron Theory in Alloy Design,The Institute of Materials,London,1992.

[23] A.Needleman,A continuum model for void nucleation by inclusion debonding,J.Appl.Mech.,ASME,Trans.54 (3) (1987)

525–531.

[24] A.S.Argon,J.Im,R.Safoglu,Cavity formation from inclusions in ductile fracture,Metal.Trans.A6 (4) (1975) 825–837.

[25] J.A.Hurtado,B.R.Elliott,H.M.Shodja,D.V.Gorelikov,C.E.Campbell,H.E.Lippard,T.C.Isabell,J.Weertman,Disclination

grain-boundary model with plastic-deformation by dislocations,Mater.Sci.Engrg.A––Struct.Mater.Propert.Microstruct.

Process.190 (1–2) (1995) 1–7.

[26] J.R.Rice,in:A.W.Thompson,I.M.Bernstein (Eds.),Eﬀect of Hydrogen on Behavior of Materials,The Metallurgical Society of

AIME,Warrendale,PA,1976,p.455.

[27] J.R.Rice,J.S.Wang,Embrittlement of interfaces by solute segregation,Mater.Sci.Engrg.A––Struct.Mater.Propert.

Microstruct.Process.107 (1989) 23–40.

[28] J.P.Hirth,J.R.Rice,On the thermodynamics of adsorption at interfaces as it inﬂuences decohesion,Metal.Trans.A––Phys.

Metal.Mater.Sci.11 (9) (1980) 1501–1511.

[29] R.J.Asaro,Adsorption-induced losses in interfacial cohesion,Philos.Trans.R.Soc.London Ser.A––Math.Phys.Engrg.Sci.

295 (1413) (1980) 151–163.

[30] I.Alber,J.L.Bassani,M.Khantha,V.Vitek,G.J.Wang,Grain boundaries as heterogeneous system atomic and continuum

elastic properties,Philos.Trans.R.Soc.London A 339 (1992) 555–586.

[31] S.Hao,W.K.Liu,B.Moran,Particle dynamics (in preparation).

[32] M.S.Daw,M.I.Baskes,Embedded-atom method––derivation and application to impurities,surfaces,and other defects in

metals,Phys.Rev.B 29 (12) (1984) 6443–6453.

[33] M.I.Baskes,Embedded atom method atomistic calculations of the dynamic interaction of an edge dislocation in nickel with

helium clusters,J.Metals 40 (11) (1988) 123.

[34] W.K.Liu,S.Jun,Y.F.Zhang,Reproducing Kernel particle methods,Int.J.Numer.Methods Fluids 20 (1995) 1081–1106.

[35] T.Belytschko,Y.Y.Lu,L.Gu,Element-free Galerkin methods,Int.J.Numer.Methods Engrg.37 (1994) 229–256.

[36] W.K.Liu,S.Jun,S.Li,J.Adee,T.Belytschko,Reproducing Kernel particle methods for structural dynamics,Int.J.Numer.

Methods Engrg.38 (1995) 1655–1680.

[37] J.T.Oden,K.Vemaganti,Adaptive hierarchical modeling of heterogeneous structures,Physica D 133 (1–4) (1999) 404–415.

[38] T.J.R.Hughes,Multiscale phenomena––Greens-functions,the Dirichlet-to-Neumann formulation,subgrid scale models,bubbles

and the origins of stabilized methods,Comput.Methods Appl.Mech.Engrg.127 (1–4) (1995) 387–401.

[39] J.S.Chen,S.P.Yoon,C.T.Wu,Non-linear version of stabilized conforming nodal integration for Galerkin mesh-free methods,

Int.J.Numer.Methods Engrg.53 (12) (2002) 2587–2615.

[40] W.K.Liu,R.A.Uras,Y.Chen,Enrichment of the ﬁnite element method with the reproducing Kernel particle method,J.Appl.

Mech.,ASME 64 (1997) 861–870.

1906 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908

[41] W.K.Liu,Y.F.Zhang,M.R.Ramirez,Multiple scale ﬁnite element methods,Int.J.Numer.Methods Engrg.32 (1991) 960–990.

[42] L.Ghosh,K.Lee,P.Raghavan,A multi-level computational model for multiscale damage analysis in composite and porous

materials,Int.J.Solids Struct.38 (14) (2001) 2335–2385.

[43] S.Hao,H.S.Park,W.K.Liu,Moving particle ﬁnite element method,In.J.Numer.Methods Engrg.53 (8) (2002) 1937–

1958.

[44] G.J.Wagner,W.K.Liu,Coupling of atomistic and continuum simulations using a bridging scale decomposition,J.Computat.

Phys.(accepted).

[45] L.E.Shilkrot,W.A.Curtin,R.E.Miller,A coupledatomistic/continuum model of defects in solids,J.Mech.Phys.Solids 50 (10)

(2002) 2085–2162.

[46] T.Belytschko,Y.Krongauz,D.Organ,M.Fleming,P.Krysl,Meshless methods:An overview and recent developments,

Comput.Methods Appl.Mech.Engrg.139 (1–4) (1996) 3–47.

[47] S.F.Li,W.K.Liu,Meshfree and particle methods and their applications,Appl.Mech.Rev.55 (2002) 1–34.

[48] T.-P.Fries,H.G.Matthies,Classiﬁcation and overview of meshfree methods,Tech.University of Braunschweig,Brunswick,

Germany,March 2003.

[49] D.J.Oh,R.A.Johnson,Simple embedded atom method model for Fcc and Hcp metals,J.Mater.Res.3 (3) (1988) 471–478.

[50] J.H.Rose,J.R.Smith,F.Guinea,J.Ferrante,Universal features of the equation of state of metals,Phys.Rev.B 29 (6) (2002)

2963–2969.

[51] R.A.Johnson,D.J.Oh,Analytic embedded atom method model for Bcc metals,J.Mater.Res.4 (5) (1989) 1195–1201.

[52] M.F.Horstemeyer et al.,A multiscale analysis of ﬁxed-end simple shear using molecular dynamics,crystal plasticity,and a

macroscopic internal state variable theory,Model.Simulat.Mater.Sci.Engrg.11 (3) (2003) 265–286.

[53] N.W.Ashcroft,N.D.Mermin,Solid State Physics,Saunders College Publishing,1976.

[54] E.B.Tadmor,M.Ortiz,R.Phillips,Quasicontinuum analysis of defects in solids,Philos.Mag.A––Phys.Cond.Matter Struct.

Defects Mech.Propert.73 (6) (1996) 1529–1563.

[55] M.Ortiz et al.,Mixed atomistic continuum models of material behavior:The art of transcending atomistics and informing

continua,MRS Bull.26 (3) (2001) 216–221.

[56] S.Hao,W.K.Liu,D.Qian,Localization-induced band and cohesive model,J.Appl.Mech.––Trans.ASME 67 (4) (2000) 803–

812.

[57] H.S.Park,W.K.Liu,An introduction and tutorial on multiple scale analysis in solids,Computat.Methods Appl.Mech.Engrg.

(accepted).

[58] D.Qian,J.Wagner,W.K.Liu,Amulti-scale projection method for the analysis of carbon nanotubes,Computat.Methods Appl.

Mech.Engrg.(accepted).

[59] W.K.Liu,K.,E.G.,Zhang,S.,Park,H.S.,An introduction to computational nanomechanics and materials,Comput.Methods

Appl.Mech.Engrg.(2003) (accepted).

[60] T.Belytschko,W.K.Liu,B.Moran,Nonlinear Finite Elements for Continua and Structures,John Wiley,Chichester New York,

2000,xvi,650.

[61] P.Zhang et al.,The elastic modulus of single-wall carbonnanotubes:a continuum analysis incorporating interatomic potentials,

Int.J.Solids Struct.39 (13-14) (2002) 3893–3906.

[62] G.B.Olson,K.C.Hsieh,Technical Report,Department of Mater Science Engineering,Northwestern University,2002.

[63] C.L.Briant,et al.,Void nucleation in a low alloy steel,in:TMS Meeting.2002.

[64] J.D.Eshelby,Elastic inclusions and inhomogeneities,in:I.N.Sneddon,R.Hill (Eds.),Progress in Solid Mechanics,North-

Holland,Amsterdam,1961,pp.89–140.

[65] R.Hill,Continuum micro-mechanics of elastoplastic polycrystals,J.Mech.Phys.Solids 13 (1965) 89–101.

[66] J.W.Hutchinson,Elastic–plastic behaviour of polycrystalline metals and composites,Proc.R.Soc.London Ser.A––Math.Phys.

Sci.319 (1537) (1970) 247.

[67] J.R.Rice,D.M.Tracey,On the ductile enlargement of voids in triaxial stress ﬁeld,J.Mech.Phys.Solids 17 (1969) 2–15.

[68] A.L.Gurson,Continuum theory of ductile rupture by void nucleation and growth:Part I––Yield criteria and ﬂow rules for

porous ductile media,J.Engrg.Mater.Technol.99 (1977) 2–15.

[69] V.Tvargaard,J.W.Hutchinson,On localization in ductile materials containing spherical voids,Int.J.Fract.18 (1982) 237–252.

[70] S.Socrate,D.M.Parks,1995,MIT,Cambridge.

[71] A.S.Khan,Y.Parikh,Astudy of 2 incremental theories of plasticity through large deformation in polycrystalline copper,Engrg.

Fract.Mech.21 (4) (1985) 697–707.

[72] B.Moran,R.J.Asaro,C.F.Shih,Eﬀects of material rate sensitivity and void nucleation on fracture initiation in a

circumferentially cracked bar,Met.Trans.22A (1991) 161–170.

[73] J.D.Embury,Damage and failure processes in structural-materials,J.Phys.IV 3 (C7) (1993) 607–619.

[74] J.M.Duva,Hutchinson,Constitutive potentials for dilutely voided non-linear materials,J.Mech.Mater.3 (1984) 41–54.

[75] A.G.Evans,M.C.Lu,S.Schmauder,M.Ruhle,Some aspects of the mechanical strength of ceramic metal bonded systems,Acta

Metal.Mater.34 (8) (1986) 1634–1655.

S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908 1907

[76] J.Fan,A micro/macroscopic analysis for cyclic plasticity of dual-phase materials,J.Appl.Mech.66 (1999) 124–130.

[77] P.Ladeveze,A damage computational method for composite structures,Comput.Struct.44 (1-2) (1992) 79–87.

[78] A.S.Khan,P.Cheng,An anisotropic elastic–plastic constitutive model for single and polycrystalline metals.II––Experiments

and predictions concerning thin-walled tubular OFHC copper,Int.J.Plast.14 (1–3) (1998) 209–226.

[79] D.L.McDowell et al.,Micro structure-based fatigue modeling of cast A356-T6 alloy,Engrg.Fract.Mech.70 (1) (2003) 49–80.

[80] P.G.Sanders,C.J.Youngdahl,J.R.Weertman,The strength of nanocrystalline metals with and without ﬂaws,Mater.Sci.Engrg.

A––Struct.Mater.Propert.Microstruct.Process.234 (1997) 77–82.

[81] T.J.R.Hughes,L.P.Franca,M.Mallet,A new ﬁnite-element formulation for computational ﬂuid-dynamics.1.Symmetrical

forms of the compressible Euler and Navier-Stokes equations and the 2nd law of thermodynamics,Comput.Methods Appl.

Mech.Engrg.54 (2) (1986) 223–234.

[82] P.Germain,Q.S.Nguyen,P.Suquet,Continuum thermodynamics,J.Appl.Mech.,ASME Trans.50 (4B) (1983) 1010–1020.

[83] J.L.Chaboche,Constitutive-equations for cyclic plasticity and cyclic viscoplasticity,Int.J.Plast.5 (3) (1989) 247–302.

[84] M.F.Horstemeyer,P.Wang,Cradle-to-grave simulation-based design incorporating multiscale microstructure-property

modeling:Reinvigorating design with science,J.Comput.Aided Mater.Design (in press).

[85] S.Hao,W.K.Liu,C.T.Chang,Computer implementation of damage models by ﬁnite element and meshfree methods,Comput.

Methods Appl.Mech.Engrg.187 (3–4) (2000) 401–440.

[86] J.F.Bishop,R.Hill,A theory of the plastic distortion of polycrystalline aggregate under combined stresses,Philos.Mag.42

(1951) 414–427.

[87] P.Klein,H.J.Gao,Crack nucleation and growth as strain localization in a virtual-bond continuum,Engrg.Fract.Mech.61

(1998) 21–48.

[88] S.Hao,W.K.Liu,P.Klein,Multi-scale damage model 2000,Chicago,IL,USA,IUTAM2000.

[89] V.Tvargaard,J.W.Hutchinson,Inﬂuence of voids on shear band instabilities under plane strain condition,Int.J.Fract.Mech.

17 (1981) 389–407.

[90] S.Hao,W.K.Liu,A.Rosakis,P.Klein,Modeling and Simulation of Intersonic Crack Growth,Northwestern University,M.

Engineering,2001.

[91] N.A.Fleck,G.M.Muller,M.F.Ashby,J.W.Hutchinson,Strain gradient plasticity:theory and experiment,Acta Metal.Mater.

42 (1994) 475–487.

[92] H.Gao,Y.Huang,W.D.Nix,J.W.Hutchinson,Mechanism-based strain gradient plasticity––I.Theory,J.Mech.Phys.Solids 47

(6) (1999) 1239–1263.

[93] V.Tvergaard,A.Needleman,Eﬀect of crack meandering on dynamic,ductile fracture,J.Mech.Phys.Solids 40 (2) (1992) 447–

471.

[95] S.Hao,W.Brocks,The Gurson–Tvergaard–Needleman-model for rate and temperature-dependent materials with isotropic and

kinematic hardening,Computat.Mech.20 (1–2) (1997) 34–40.

[96] S.Hao,W.K.Liu,Moving particle ﬁnite element method with global superconvergence (submitted).

[97] B.Moran,F.Shih,Crack tip and associated domain integrals from momentum and energy-balance,Engrg.Fract.Mech.27 (6)

(1987) 615–642.

[98] B.Moran,F.Shih,A general treatment of crack tip contour integrals,Int.J.Fract.35 (4) (1987) 295–310.

[99] P.G.Mcdougall,G.B.Olson,M.Cohen,Interphase crystallography and interfacial structure,J.Metals 35 (12) (1983) 17.

[100] J.D.Landes,K.Brown,Results from a round robin on a standard method for measurement of fracture toughness,J.Testing

Evaluat.26 (4) (1998) 396–403.

[101] K.H.Schwalbe,Inﬂuence of microstructure on crack-propagation mechanisms and fracture toughness of metallic materials,

Engrg.Fract.Mech.9 (4) (1977) 795–832.

[102] A.Saxena,Creep crack-growth in high-temperature ductile materials,Engrg.Fract.Mech.40 (4–5) (1991) 721–736.

[103] R.Gaspar,Acta Phys.Acad.Sci.Hung.3 (1954) 263.

[104] L.Heidin,S.J.Lundqvist,Phys.(France) 33 (C3-73) (1972).

[105] T.J.R.Hughes,J.Winget,Finite rotation eﬀects in numerical integration of rate constitutive equations arising in large-

deformation analysis,Int.J.Numer.Methods Engrg.15 (1980) 1862–1867.

[106] M.F.Horstemeyer,M.I.Baskes,Atomistic ﬁnite deformation simulations:a discussion on length scale eﬀects in relation to

mechanical stresses,J.Engrg.Mater.Technol.––Trans.ASME 121 (2) (1999) 114–119.

[107] A.S.Khan,X.M.Su,Constitutive relations for single-crystal based on 2 surface description,Int.J.Plast.10 (7) (1994) 807–823.

[108] A.S.Khan,Y.Parikh,Large deformation in polycrystalline copper under combined tension–torsion,loading,unloading and

reloading or reverse loading––a study of 2 incremental theories of plasticity,Int.J.Plast.2 (4) (1986) 379–392.

[109] E.H.Lee,Elastic–plastic deformation at ﬁnite strain,J.Appl.Mech.36 (1969) 1–6.

1908 S.Hao et al./Comput.Methods Appl.Mech.Engrg.193 (2004) 1865–1908

## Comments 0

Log in to post a comment